Upcoming SlideShare
×

# Theory of electroelasticity

471
-1

Published on

0 Likes
Statistics
Notes
• Full Name
Comment goes here.

Are you sure you want to Yes No
• Be the first to comment

• Be the first to like this

Views
Total Views
471
On Slideshare
0
From Embeds
0
Number of Embeds
0
Actions
Shares
0
0
0
Likes
0
Embeds 0
No embeds

No notes for slide

### Theory of electroelasticity

1. 1. Chapter 7 Three-Dimensional and Applied Electroelastic Problems Abstract In this chapter, there are mainly two kinds of problems discussed. The ﬁrst kind of problems is the 3D electroelastic problems: the potential function method, the solutions of the penny-shaped crack and elliptic inclusions. The second kind of problems is the applied electroelastic problems which are used in engineer- ing: simple electroelastic problems, laminated piezoelectric plates containing clas- sical and higher-order theories and piezoelectric composite shells. A uniﬁed ﬁrst- order approximate theory of an electro-magneto-elastic thin plate derived by the physical variational principle is given when the electromagnetic induction effect can be neglected. Keywords Penny-shaped crack • Laminated piezoelectric plate • Piezoelectric composite shell 7.1 Potential Function Methods in Transversely Isotropic Piezoelectric Materials 7.1.1 Governing Equations The governing equations of transversely isotropic piezoelectric materials have been discussed in previous chapters. In the material principle coordinates, the constitutive equations are σ1 ¼ C11u1;1 þ C12u2;2 þ C13u3;3 þ e31φ;3; σ2 ¼ C12u1;1 þ C11u2;2 þ C13u3;3 þ e31φ;3 σ3 ¼ C13u1;1 þ C13u2;2 þ C33u3;3 þ e33φ;3; σ4 ¼ σ23 ¼ C44ðu2;3 þ u3;2Þ þ e15φ;2 σ5 ¼ σ31 ¼ C44ðu1;3 þ u3;1Þ þ e15φ;1; σ6 ¼ σ12 ¼ C66ðu2;1 þ u1;2Þ D1 ¼ e15ðu1;3 þ u3;1Þ À E11φ;1; D2 ¼ e24ðu2;3 þ u3;2Þ À E11φ;1 D3 ¼ e31u1;1 þ e31u2;2 þ e33u3;3 À E33φ;3; C66 ¼ ðC11 À C12Þ 2= (7.1) Z.-B. Kuang, Theory of Electroelasticity, DOI 10.1007/978-3-642-36291-0_7, © Shanghai Jiao Tong University Press, Shanghai and Springer-Verlag Berlin Heidelberg 2014 339
2. 2. The generalized momentum equations are σ1;1 þ σ6;2 þ σ5;3 ¼ ρ€u1; σ6;1 þ σ2;2 þ σ4;3 ¼ ρ€u2; σ5;1 þ σ4;2 þ σ3;3 ¼ ρ€u3 D1;1 þ D2;2 þ D3;3 ¼ 0 (7.2) where i ¼ 1; 2; 3. Substitution of Eq. (7.1) into Eq. (7.2) yields C11u1;11 þ C66u1;22 þ C44u1;33 þ ðC12 þ C66Þu2;12 þ ðC13 þ C44Þu3;13 þ ðe15 þ e31Þφ;13 ¼ ρu1;tt ðC12 þ C66Þu1;12 þ C66u2;11 þ C11u2;22 þ C44u2;33 þ ðC13 þ C44Þu3;23 þ ðe15 þ e31Þφ;23 ¼ ρu2;tt ðC13 þ C44Þðu1;13 þ u2;23Þ þ C44r2 u3 þ C33u3;33 þ e15r2 φ þ e33φ;33 ¼ ρu3;tt ðe15 þ e31Þðu1;13 þ u2;23Þ þ e15r2 u3 þ e33u3;33 À E11r2 φ À E33φ;33 ¼ 0 r2 u ¼ u;11 þ u;22 (7.3) 7.1.2 General Solution of the Static Problem (I) Wang and Zheng (1995) discussed the general solution of (7.3) for the static problem by introducing potential functions. They assume u1 ¼ ψ;1 À χ;2; u2 ¼ ψ;2 þ χ;1; u3 ¼ k1ψ;3; φ ¼ k2ψ;3 (7.4) where k1 and k2 are undetermined constants and ψ and χ are potential functions. Substitution of Eq. (7.4) into Eq. (7.3) yields C66r2 χ þ C44χ;33 ¼ 0; or r2 χ þ @2 χ @z2 0 ¼ 0; z0 ¼ s0x3; s2 0 ¼ C66 C44= ¼ 1 λ0= (7.5) C11r2 ψ þ C44 þ k1 C13 þ C44ð Þ þ k2 e15 þ e31ð Þ½ ψ;33 ¼ 0 ðC13 þ C44Þ þ k1C44 þ k2e15½ r2 ψ þ k1C33 þ k2e33ð Þψ;33 ¼ 0 ðe15 þ e31Þ þ k1e33 À k2 E11½ r2 ψ þ k1e33 À k2 E33ð Þψ;33 ¼ 0 (7.6) In order to have nontrivial solution of Eq. (7.6), the following relations must be held: C44 þ k1ðC13 þ C44Þ þ k2ðe15 þ e31Þ C11 ¼ k1C33 þ k2e33 ðC13 þ C44Þ þ k1C44 þ k2e15 ¼ k1e33 À k2 E33 ðe15 þ e31Þ þ k1e33 À k2 E11 ¼ λ (7.7) 340 7 Three-Dimensional and Applied Electroelastic Problems
3. 3. Eliminating k1 and k2, a cubic algebra equation of λ is obtained: Aλ3 þ Bλ2 þ Cλ þ D ¼ 0 A ¼ e2 15 þ C44 E11; D ¼ ÀCÀ1 11 e2 33C44 þ E33C11C33 À Á B ¼ CÀ1 11 2e2 15C13 À e2 31C44 þ 2e15ðe31C13 À e33C11Þ þ E11 C2 13 þ 2C13C44 À ÁÈ À E11C11C33ÀE33C11C44g C ¼ CÀ1 11 ðe15 þ e31Þ2 C33 À 2e33ðe15 þ e31ÞðC13 þ C44Þ À ðC13 þ C44ÞÀ1 ðe15 þ e31ÞC33½ n Àðe15 þ e11ÞC11C44e15 þ E11C44C33 þ e2 33C11 À E33 C13 þ C44ð Þ2 þ E33 C2 44 þ C11C33 À ÁÉ (7.8) Assume root λ1 is positive real and λ2 and λ3 are either a pair of conjugate complex roots with positive real parts or positive real roots. Corresponding to each λi, a potential function ψj in Eq. (7.6) can be obtained: r2 ψj þ λj @2 ψj @x2 3 ¼ r2 ψj þ @2 ψj @z2 j ¼ 0; zj ¼ sjx3; s2 j ¼ 1 λj ; j ¼ 1; 2; 3 (7.9) Substituting λj into Eq. (7.7), k1j and k2j can be obtained. So the general solution of Eq. (7.3) can be expressed in potential functions: u1 ¼ ðψ1 þ ψ2 þ ψ3Þ;1 À χ;2; u2 ¼ ðψ1 þ ψ2 þ ψ3Þ;2 þ χ;1; u3 ¼ k11ψ1;3 þ k12ψ2;3 þ k13ψ3;3; φ ¼ k21ψ1;3 þ k22ψ2;3 þ k23ψ3;3 (7.10) Usually the numerical method is used to solve λj in Eq. (7.8) due to its complex roots. As an example for material PZT-6B with material constants, C11 ¼ 168 MPað Þ; C33 ¼ 163; C44 ¼ 27:1; C12 ¼ 60; C13 ¼ 60 e31 ¼ À0:9 C m2 À Á ; e33 ¼ 7:1; e15 ¼ 4:6; E11 ¼ 36 Â 10À10 F m=ð Þ; E33 ¼ 34 Â 10À10 The solved λ is λ1 ¼ 3:92; λ2 ¼ 0:73 þ 0:87i; λ3 ¼ 0:73 À 0:87i. 7.1.3 General Solution of the Dynamic Problem Ding et al. (1996) discussed the dynamic problem. Let u1 ¼ ψ;2 À χ;1; u2 ¼ Àψ;1 À χ;2 (7.11) where ψ and χ are potential functions, but their meanings are different with that in Sect. 7.1.2. Substituting Eq. (7.11) into the ﬁrst two equations in Eq. (7.3) yields 7.1 Potential Function Methods in Transversely Isotropic Piezoelectric Materials 341
4. 4. B;2 À A;1 ¼ 0; B;1 þ A;2 ¼ 0; B ¼ C66r2 ψ þ C44ψ;33 À ρψ;tt A ¼ C11r2 χ þ C44χ;33 À ρχ;tt À ðC13 þ C44Þu3;3 À ðe15 þ e31Þφ;3 (7.12) Let A ¼ H;2; B ¼ H;1,and Eq. (7.12) is reduced to r2 H ¼ 0. One particular solution is H ¼ constant. Adopt a particular solution A ¼ 0; B ¼ 0 (7.13) Using this result, substituting Eq. (7.11) into the last two equations in Eq. (7.3) and listing the results with Eq. (7.13) together we get C66r2 ψ þ C44ψ;33 À ρψ;tt ¼ 0 (7.14) DG ¼ 0; G ¼ χ; u3; φ½ T D ¼ C11r2 þ C44 @2 @x2 3 À ρ @2 @t2 À C13 þ C44ð Þ @ @x3 À e15 þ e31ð Þ @ @x3 À C13 þ C44ð Þr2 @ @x3 C44r2 þ C33 @2 @x2 3 À ρ @2 @t2 e15r2 þ e33 @2 @x2 3 e15 þ e31ð Þr2 @ @x3 À e15r2 þ e33 @2 @x2 3 E11r2 þ E33 @2 @x2 3 0 B B B B B B B B @ 1 C C C C C C C C A (7.15) Introduce a new function F and let Dj jF ¼ 0 or Dj jF ¼ a @6 @x6 3 þ br2 @4 @x4 3 þ cr4 @2 @x2 3 þ dr6 þ gr2 @4 @t4 þ hr4 @2 @t2 þ kr2 @2 @x2 3 @2 @t2 þ l @4 @x4 3 @2 @t2 þm @2 @x2 3 @4 @t4 ' F ¼ 0 (7.16) where a ¼ C44 e2 33 þ C33E33 À Á b ¼ C33 C44E11 þ ðe15 þ e31Þ2 h i þ E33 C11C33 þ C2 44 À ðC13 þ C44Þ2 h i þ e33 2C44e15 þ C11e33 À 2ðC13 þ C44Þðe15 þ e31Þ½  c ¼ C44 C11 E33 þ ðe15 þ e31Þ2 h i þ E11 C11C33 þ C2 44 À ðC13 þ C44Þ2 h i þ e15 2C11e33 þ C44e15 À 2ðC13 þ C44Þðe15 þ e31Þ½  d ¼ C11 e2 15 þ C44E11 À Á ; g ¼ ρ2 E11; h ¼ Àρ e2 15 þ ðC11 þ C44ÞE11 Â Ã k ¼ Àρ 2e15e33 þ ðC33 þ C44Þ E11 þ ðC11 þ C44ÞE33 þ ðe15 þ e31Þ2 h i l ¼ Àρ e2 33 þ ðC33 þ C44ÞE33 Â Ã ; m ¼ ρ2 E33 (7.17) 342 7 Three-Dimensional and Applied Electroelastic Problems
5. 5. After solving F, it can be proved that the three group solutions of χ; u3; φ are χ ¼ Ai1F; u3 ¼ Ai2F; φ ¼ Ai3F; i ¼ 1; 2; 3 (7.18) where Aij in Eq. (7.18) is the algebraic complement of Dj j, i.e., A11 ¼ C44r2 þ C33 @2 @x2 3 À ρ @2 @t2 E11r2 þ E33 @2 @x2 3 þ e15r2 þ e33 @2 @x2 3 2 A12 ¼ E11r2 þ E33 @2 @x2 3 ðC13 þ C44Þ þ e15r2 þ e33 @2 @x2 3 ðe15 þ e31Þ ! r2 @ @x3 A13 ¼ e15r2 þ e33 @2 @x2 3 ðC13 þ C44Þ À C44r2 þ C33 @2 @x2 3 À ρ @2 @t2 ðe15 þ e31Þ ! r2 @ @x3 (7.19) A21 ¼ E11r2 þ E33 @2 @x2 3 ðC13 þ C44Þ þ e15r2 þ e33 @2 @x2 3 ðe15 þ e31Þ ! @ @x3 A22 ¼ C11r2 þ C44 @2 @x2 3 À ρ @2 @t2 E11r2 þ E33 @2 @x2 3 þ ðe15 þ e31Þ2 r2 @2 @x2 3 A23 ¼ C11r2 þ C44 @2 @x2 3 À ρ @2 @t2 e15r2 þ e33 @2 @x2 3 À ðC13 þ C44Þðe15 þ e31Þr2 @2 @x2 3 (7.20) A31 ¼ C44r2 þ C33 @2 @x2 3 À ρ @2 @t2 ðe15 þ e31Þ À e15r2 þ e33 @2 @x2 3 ðC13 þ C44Þ ! @ @x3 A32 ¼ ðe15 þ e31ÞðC13 þ C44Þr2 @2 @x2 3 À C11r2 þ C44 @2 @x2 3 À ρ @2 @t2 e15r2 þ e33 @2 @x2 3 A33 ¼ C11r2 þ C44 @2 @x2 3 À ρ @2 @t2 C44r2 þ C33 @2 @x2 3 À ρ @2 @t2 À ðC13 þ C44Þ2 r2 @2 @x2 3 (7.21) By substitution of Eq. (7.18) into Eq. (7.11), the general solution is u1 ¼ ψ;2 À Ai1F;1; u2 ¼ Àψ;1 À Ai1F;2; u3 ¼ Ai2F; φ ¼ Ai3F; i ¼ 1; 2; 3 (7.22) The general solution of an axial-symmetric problem can be obtained from Eq. (7.22) if let ψ ¼ 0 and F is independent of θ. 7.1.4 General Solution of the Static Problem (II) Let all the potential functions be independent of the time the general solution of the static problem can be obtained from the results in Sect. 7.1.3. Equation (7.14) yields r2 þ @2 @z2 0 À Á ψ0 ¼ 0 z2 0 ¼ s2 0x2 3; s2 0 ¼ C66 C44= (7.23) 7.1 Potential Function Methods in Transversely Isotropic Piezoelectric Materials 343
6. 6. Equation (7.16) can be reduced to r2 þ @2 @z2 1 r2 þ @2 @z2 2 r2 þ @2 @z2 3 F ¼ 0 z2 i ¼ s2 i x2 3; i ¼ 1; 2; 3 (7.24) where s2 i is the root of the following equation: as6 À bs4 þ cs2 À d ¼ 0 (7.25) No loss of generality let s1 be real and assume Re sið Þ 0. It is easy to prove that Fi satisfying the following equation is the solution of Eq. (7.24): r2 þ @2 @z2 i Fi ¼ 0; z2 i ¼ s2 i x2 3; i ¼ 1; 2; 3 (7.26) The general solutions of Eq. (7.24) are 1. s2 1 6¼ s2 2 6¼ s2 3; F ¼ F1 þ F2 þ F3 (7.27) 2. s2 1 6¼ s2 2 ¼ s2 3 F ¼ F1 þ F2 þ x3F3 (7.28a) 3. s2 1 ¼ s2 2 ¼ s2 3; F ¼ F1 þ x3F2 þ x2 3F3; (7.28b) From Eq. (7.26), it is obtained that r2 ¼ À@2 @z2 i ; @ @x3= ¼ si@ @zi= . Substituting these results into Eq. (7.20) yields A21 ¼ β1r2 þ β2 @2 @x2 3 @ @x3 ¼ ðβ2s2 i À β1Þsi @3 @z3 i A22 ¼ C11 E11r4 þ β3r2 @2 @x2 3 þ C44 E33 @4 @x4 3 ¼ C44 E33s4 i À β3s2 i þ C11 E11 À Á @4 @z4 i A23 ¼ C11e15r4 þ β4r2 @2 @x2 3 þ C44e33 @4 @z4 3 ¼ C44e33s4 i À β4s2 i þ C11e15 À Á @4 @z4 i β1 ¼ E11ðC13 þ C44Þ þ e15ðe15 þ e31Þ; β2 ¼ E33ðC13 þ C44Þ þ e33ðe15 þ e31Þ β3 ¼ C11E33 þ C44E11 þ ðe15 þ e31Þ2 ; β4 ¼ C11e33 þ C44e15 À ðC13 þ C44Þðe15 þ e31Þ (7.29) The general solution Eq. (7.22) can be rewritten as u1 ¼ @ψ @x2 þ X3 i¼1 αi1si @4 Fi @x1@z3 i ; u2 ¼ À @ψ @x1 þ X3 i¼1 αi1si @4 Fi @x2@z3 1 ; u3 ¼ X3 i¼1 αi2 @4 Fi @z4 i ; φ ¼ X3 i¼1 αi3 @4 Fi @z4 i αi1 ¼ β1 À β2s2 i ; αi2 ¼ C11 E11 À β3s2 i þ C44 E33s4 i ; αi3 ¼ C11e15 À β4s2 i þ C44e33s4 i (7.30) 344 7 Three-Dimensional and Applied Electroelastic Problems
7. 7. If let α1isi@3 Fi @z3 i ¼ ψi; ψ0 ¼ Àψ, Eq. (7.30) can be reduced to u1 ¼ À @ψ0 @x2 þ X3 i¼1 @ψi @x1 ; u2 ¼ @ψ0 @x1 þ X3 i¼1 @ψi @x2 ; u3 ¼ X3 i¼1 ki1 @ψi @zi φ ¼ X3 i¼1 ki2 @ψi @zi ; ki1 ¼ αi2 αi1si= ; ki2 ¼ αi3 αi1si= (7.31) Equations (7.31) and (7.10) are formally the same. 7.2 A Penny-Shaped Crack in Transversely Isotropic Material 7.2.1 Governing Equations Consider a transversely isotropic piezoelectric material weakened by a ﬂat imper- meable crack of radius a occupied region S in the plane x3 ¼ 0, subjected to distributed pressure À p x1; x2ð Þ and surface electric charge q x1; x2ð Þ (Fig. 7.1). In Fig. 7.1 only a pair of concentrated force and electric charge is shown. The Cartesian coordinates x1; x2; x3ð Þ and cylindrical coordinates r; θ; zð Þ are adopted simultaneously. Using the symmetry with respect to the crack surface, this problem can be reduced to a mixed boundary value problem for a half space subjected to the following boundary conditions: σ33 ¼ Àpðx1; x2Þ; D3 ¼ qðx1; x2Þ; when ðx1; x2Þ 2 S u3 ¼ φ ¼ 0; when ðx1; x2Þ =2 S; σ31 ¼ σ32 ¼ 0; À1 ðx1; x2Þ 1 (7.32) Chen and Shioya (1999) extended the method proposed by Fabrikant (1989) in the elasticity, to solve above problem. Introduce notation Λ ¼ @ @x1= þ i@ @x2= and complex displacement U ¼ u1 þ iu2 . Let w ¼ x3 , the generalized momentum equations in complex displacement is ð1 2= ÞðC11 þ C66Þr2 U þ C44U;33 þ ð1 2= ÞðC11 À C66ÞΛ2 U þ ðC13 þ C44ÞΛw;3 þ ðe15 þ e31ÞΛφ;3 ¼ 0 ð1 2= ÞðC13 þ C44Þ ΛU þ Λ Uð Þ;3þC44r2 w þ C33w;33 þ e15r2 φ þ e33φ;33 ¼ 0 ð1 2= Þðe15 þ e31Þ ΛU þ Λ Uð Þ;3 þ e15r2 w þ e33w;33 À E11r2 φ À E33φ;33 ¼ 0 (7.33) 7.2 A Penny-Shaped Crack in Transversely Isotropic Material 345
8. 8. where U; Λ mean the conjugate value of U; Λ. By using the complex displacement, the general solution in potential functions, Eq. (7.31), become U ¼ Λ X3 i¼1 ψi þ iψ0 ! ; w ¼ X3 i¼1 ki1 @ψi @zi ; φ ¼ X3 i¼1 ki2 @ψi @zi (7.34) The generalized stresses become σ11 þ σ22 ¼ 2r2 X3 i¼1 ðC11 À C66 À C13siki1 À e31siki2Þψi σ11 À σ22 þ 2iσ12 ¼ 2C66Λ2 ðψ1 þ ψ2 þ ψ3 þ iψ0Þ σ31 þ iσ32 ¼ Λ X3 i¼1 C44ðki1 þ siÞ þ e15ki2½  @ψi @zi þ is4C44 @ψ0 @z0 ( ) D1 þ iD2 ¼ Λ X3 i¼1 e15ðki1 þ siÞ À E11ki2½  @ψi @zi þ is4e15 @ψ0 @z0 ( ) σ33 ¼ Àr2 X3 i¼1 γ1iψi; D3 ¼ Àr2 X3 i¼1 γ2iψi; r2 ¼ À@2 @z2 i γ1i ¼ ÀC13 þ C33siki1 þ e33siki2; γ2i ¼ Àe31 þ e33siki1 À E33siki2 (7.35) where si is the root of the Eq. (7.25). Fig. 7.1 A penny-shaped crack in a transversely isotropic piezoelectric material 346 7 Three-Dimensional and Applied Electroelastic Problems
9. 9. 7.2.2 Potential Theory Method of Crack Problem The solution satisfying the boundary conditions in Eq. (7.32) can be expressed by two harmonic functions G and H: ψiðziÞ ¼ ciGðziÞ þ diHðziÞ; i ¼ 1; 2; 3; ψ0ðz0Þ ¼ 0 (7.36) where ci; di are undetermined constants. G and H can be expressed by two potentials of a simple layer: Gðr; θ; zÞ ¼ Z S ^uðNÞ ρðM; NÞ dS; Hðr; θ; zÞ ¼ Z S ^φðNÞ ρðM; NÞ dS (7.37) where ^uðNÞ ¼ wðx1; x2; 0Þ and ^φðNÞ ¼ ^φðx1; x2; 0Þ are undetermined displace- ment and electric potential on the crack surface, respectively. Nðr1; θ1; 0Þ is a point on S, Mðr; θ; zÞ is a certain point in the material, and ρðM; NÞ is the distance between N and M. According to the property of the potential of a simple layer, the boundary conditions w ¼ φ ¼ 0 outside the crack in Eq. (7.37) are satisﬁed automatically. Inside the crack we have ð@G @z= Þz¼0 ¼ À2π^u; ð@H @z= Þz¼0 ¼ À2π^φ (7.38) Equations (7.34), (7.36), and (7.38) yield X3 i¼1 ciki1 ¼ À 1 2π ; X3 i¼1 diki1 ¼ 0; X3 i¼1 ciki2 ¼ 0; X3 i¼1 diki2 ¼ À 1 2π (7.39) The boundary conditions of σ31; σ32 in Eq. (7.32) demand X3 i¼1 ci C44ðki1 þ siÞ þ e15ki2½  ¼ 0; X3 i¼1 di C44ðki1 þ siÞ þ e15ki2½  ¼ 0 (7.40) Combining Eqs. (7.39) and (7.40) yields c1 c2 c3 8 : 9 = ; ¼ 1 2π s1 s2 s3 k11 k21 k31 k12 k22 k32 0 B @ 1 C A À1 1 À 1 0 8 : 9 = ; ; d1 d2 d3 8 : 9 = ; ¼ 1 2π s1 s2 s3 k11 k21 k31 k12 k22 k32 0 B @ 1 C A À1 e15 C44= 0 À 1 8 : 9 = ; (7.41) 7.2 A Penny-Shaped Crack in Transversely Isotropic Material 347
10. 10. ^uðNÞ and ^φðNÞ can be determined from the ﬁrst two boundary conditions in Eq. (7.32): pðN0Þ ¼ Àη1r2 ð ð S ^uðNÞ ρðN0; NÞ dS À η2r2 ð ð S ^φðNÞ ρðN0; NÞ dS; qðN0Þ ¼ Àη3r2 ð ð S ^uðNÞ ρðN0; NÞ dS À η4r2 ð ð S ^φðNÞ ρðN0; NÞ dS η1 ¼ À X3 i¼1 ciγ1i; η2 ¼ À X3 i¼1 diγ1i; η3 ¼ X3 i¼1 ciγ2i; η4 ¼ X3 i¼1 diγ2i (7.42) where N0ðr0; θ0; 0Þ; Nðr1; θ1; 0Þ 2 S and the integral is over all points on S . Equation (7.42) yields η4pðN0Þ À η2qðN0Þ ¼ À 1 4π2A r2 ð ð S ^uðNÞ ρðN0; NÞ dS η1qðN0Þ À η3pðN0Þ ¼ À 1 4π2A r2 ð ð S ^φðNÞ ρðN0; NÞ dS; A ¼ 1 4π2 ðη1η4 À η2η3Þ (7.43) Equation (7.43) can be applied for a crack with any shape. 7.2.3 The Solution of a Circular Penny-Shaped Crack For a circular penny-shaped crack of diameter 2a, the solution of Eq. (7.43) is ^u ¼ 2A π Z 2π 0 Z a 0 1 ρ arc tan ξ ρ η4pðr0; θ0Þ À η2qðr0; θ0Þ½ r0dr0dθ0 ^φ ¼ 2A π Z 2π 0 Z a 0 1 ρ arc tan ξ ρ η1qðr0; θ0Þ À η3pðr0; θ0Þ½ r0dr0dθ0 ρ ¼ ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ r2 1 þ r2 0 À 2r1r0 cosðθ À θ0Þ q ; ξ ¼ ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ða2 À r2 1Þða2 À r2 0Þ q 0 a (7.44) Substituting Eq. (7.44) into (7.37) yields Gðr; θ; zÞ ¼ 2A π Z 2π 0 Z a 0 K r; θ; z; r0; θ0ð Þ η4pðr0; θ0Þ À η2qðr0; θ0Þ½ r0dr0dθ0 Hðr; θ; zÞ ¼ 2A π Z 2π 0 Z a 0 K r; θ; z; r0; θ0ð Þ η1qðr0; θ0Þ À η3pðr0; θ0Þ½ r0dr0dθ0 (7.45) 348 7 Three-Dimensional and Applied Electroelastic Problems
11. 11. The kernel function K in Eq. (7.45) is KðM; N0Þ ¼ Z 2π 0 Z a 0 1 ρðN; N0Þ arc tan ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ a2 À r2ð Þ a2 À r2 0 À Áq aρðN; N0Þ 2 4 3 5 r1dr1dθ1 ρðM; NÞ KðM; N0Þ ¼ Kðr; θ; z; r0; θ0Þ (7.46) Using the relation @K @z= ¼ À 2π ρðM; N0Þ=½  arctan h ρðM; N0Þ=½  (Fabrikant 1989), the derivatives of G and H in Eq. (7.45) are @G @z ¼ À4A Z 2π 0 Z a 0 1 ρðM; N0Þ arc tan h ρðM; N0Þ ! η4pðr0; θ0Þ À η2qðr0; θ0Þ½ r0dr0dθ0 @H @z ¼ À4A Z 2π 0 Z a 0 1 ρðM; N0Þ arc tan h ρðM; N0Þ ! η1qðr0; θ0Þ À η3pðr0; θ0Þ½ r0dr0dθ0 h ¼ ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ a2 À l2ð Þ a2 À r2 0 À Áq a= ; l ¼ ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ðr þ aÞ2 þ z2 q À ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ðr À aÞ2 þ z2 q '0 2 (7.47) So for arbitrary polynomial distributed loadings p and q, all the generalized stresses can be expressed by elementary functions. 7.2.4 A Circular Penny-Shaped Crack Subjected to Generalized Concentrate Loading Assume the penny-shaped crack is subjected to a pair of normal concentrated generalized loading ÀP; Qð Þ at point r0; θ0; 0Æ ð Þ; r0 a (Fig. 7.1). By using the general solution in the above section, after some manipulation, the generalized displacements and stresses can be obtained as u ¼ 4A X3 i¼1 τi1f1ðziÞP þ τi2f1ðziÞQ½  u3 ¼ À4A X3 i¼1 ki1 τi1f2ðziÞP þ τi2f2ðziÞQ½  φ ¼ À4A X3 i¼1 ki2 τi1f2ðziÞP þ τi2f2ðziÞQ½  σ33 ¼ 4A X3 i¼1 γ1i τi1f3ðziÞP þ τi2f3ðziÞQ½  D3 ¼ 4A X3 i¼1 γ2i τi1f3ðziÞP þ τi2f3ðziÞQ½  (7.48a) 7.2 A Penny-Shaped Crack in Transversely Isotropic Material 349
12. 12. where f1ðziÞ ¼ 1 t0 zi R0 arc tan h0 R0 À ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ a2 À r2 0 p α0 arc tan α0 ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ m2 À a2 p ( ) ; f2ðziÞ ¼ 1 R0 arc tan h0 R0 f3ðziÞ ¼ 1 R0 arc tan h0 R0 À h0 zi R2 0 þ h2 0 À Á r2 À l2 m2 À l2 À z2 j R2 0 ! ; α0 ¼ ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ a2 À rr0eÀiðθÀθ0Þ p R0 ¼ ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ r2 þ r2 0 À 2rr0 cosðθ À θ0Þ þ z2 q ; m ¼ 1 2 ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ðr þ aÞ2 þ z2 q þ ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ðr À aÞ2 þ z2 q ' τi1 ¼ ciη4 À diη3; τi2 ¼ diη1 À ciη2; h0 ¼ ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ a2 À l2ð Þ a2 À r2 0 À Áq 0 a; t0 ¼ reÀiθ À r0eÀiθ0 (7.48b) The generalized stress intensity factors are KI ¼ P π3 2= ﬃﬃﬃ a p ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ a2 À r2 0 p a2 þ r2 0 À 2ar0 cosðθ À θ0Þ ; KD ¼ Q π3 2= ﬃﬃﬃ a p ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ a2 À r2 0 p a2 þ r2 0 À 2ar0 cosðθ À θ0Þ (7.49) For the distributed loadings Àp; qð Þ, the generalized stress intensity factors are KI ¼ ﬃﬃﬃﬃﬃ 2π p π2 ﬃﬃﬃﬃﬃ 2a p Z 2π 0 Z a 0 pðr0; θ0Þ ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ a2 À r2 0 p a2 þ r2 0 À 2ar0 cosðθ À θ0Þ r0dr0dθ0 KD ¼ ﬃﬃﬃﬃﬃ 2π p π2 ﬃﬃﬃﬃﬃ 2a p Z 2π 0 Z a 0 qðr0; θ0Þ ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ a2 À r2 0 p a2 þ r2 0 À 2ar0 cosðθ À θ0Þ r0dr0dθ0 (7.50) For homogeneous distributed loadings Àp0; D30ð Þ, the generalized stress intensity factors are KI ¼ 2p0 ﬃﬃﬃﬃﬃﬃﬃﬃ a π= p ; KD ¼ 2D30 ﬃﬃﬃﬃﬃﬃﬃﬃ a π= p (7.51) From Eq.(7.51), it is seenthat the stress intensity factoris determinedindependently by the mechanical loading and the electric displacement intensity factor is determined independently bytheelectric loading.Equation(7.51) obviously can be used tothecase where homogeneous generalized stresses σ33 and À D3 are applied at inﬁnity. There are many papers to discuss the penny-shaped crack, such as Huang (1997) and Wang (1992). 7.2.5 A Conducting Penny-Shaped Crack Chen and Lim (2005) discussed the conducting penny-shaped crack. For a conducting crack, it adopts φ ¼ 0 instead of D3 ¼ qðx1; x2Þ in Eq. (7.32). The boundary conditions are 350 7 Three-Dimensional and Applied Electroelastic Problems
13. 13. σ33 ¼ Àpðx1; x2Þ; when ðx1; x2Þ 2 S; w ¼ 0; when ðx1; x2Þ =2 S φ ¼ 0; σ31 ¼ σ32 ¼ 0; À 1 ðx1; x2Þ 1 (7.52) According toφ ¼ 0; À1 ðx1; x2Þ 1 in Eq. (7.52), it is concluded thatH ¼ 0 in Eqs. (7.36) and (7.37). Equation (7.42) becomes pðN0Þ ¼ Àη1r2 ð ð S ^uðNÞ ρðN0; NÞ dS; η1 ¼ À X3 i¼1 ciγ1i (7.53) Equation (7.45) is reduced to G r; θ; zð Þ ¼ 1 2π3η1 Z 2π 0 Z a 0 K r; θ; z; r0; θ0ð Þpðr0; θ0Þr0dr0dθ0 (7.54) where K r; θ; z; r0; θ0ð Þ is still expressed by Eq. (7.46). The generalized displace- ments and stresses for a circular penny-shaped crack subjected to a concentrated force À P are U ¼ P π2η1 X3 i¼1 cif1ðziÞ; u3 ¼ À P π2η1 X3 i¼1 ki1cif2ðziÞ; φ ¼ À P π2η1 X3 i¼1 ki2cif2ðziÞ σ33 ¼ P π2η1 X3 i¼1 γ1icif3ðziÞ; D3 ¼ P π2η1 X3 i¼1 γ2icif3ðziÞ (7.55) The functions in Eq. (7.55) are still expressed by Eq. (7.48b). The generalized stress intensity factors are KI ¼ P π3=2 ﬃﬃﬃ a p ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ a2 À r2 0 p a2 þ r2 0 À 2ar0 cosðθ À θ0Þ ; KD ¼ β π3=2 ﬃﬃﬃ a p ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ a2 À r2 0 p a2 þ r2 0 À 2ar0 cosðθ À θ0Þ (7.56) where β ¼ À P3 i¼1 γi1ci η1= . Above results are assumed that Eq. (7.27) or Eq. (7.24) has three different roots, si; i ¼ 1; 2; 3 . Chen and Lim (2005) also discussed other cases. 7.2.6 Solve an Impermeable Penny-Shaped Crack by Hankel Transform In order to discuss the results of the Vickers indentation cracking of experiments, Jiang and Sun (2001) gave a solution of an impermeable penny-shaped crack with 7.2 A Penny-Shaped Crack in Transversely Isotropic Material 351
14. 14. boundary conditions as shown in Eq. (7.32). They discussed an axisymmetric piezoelectric body under axisymmetric loading by using the Hankel transform method in cylindrical coordinates. In cylindrical coordinates, the constitutive equations are σr σϑ σz τrz Dr Dz 8 : 9 = ; ¼ C11 C12 C13 0 0 Àe31 C12 C11 C13 0 0 Àe31 C13 C13 C33 0 0 Àe33 0 0 0 C44 Àe15 0 0 0 0 e15 E11 0 e31 e31 e33 0 0 E33 2 6 6 6 6 6 6 6 6 6 4 3 7 7 7 7 7 7 7 7 7 5 εr εϑ εz γrz Er Ez 8 : 9 = ; (7.57) The generalized geometric equations are εr ¼ u;r; εϑ ¼ u r= ; εz ¼ w;z; γrz ¼ u;z þ w;r; Er ¼ Àφ;r; Ez ¼ Àφ;z (7.58) where u; w are the displacements along r; z directions, respectively. The generalized equilibrium equations are σr;r þ τrz;z þ ðσr À σϑÞ r= ¼ 0; τrz;r þ σz;z þ τrz r= ¼ 0; @ðrDrÞ @r= þ r @ðDzÞ @z= ¼ 0 (7.59) or C11 u;rr þ 1 r u;r À u r2 þ C44u;zz þ ðC13 þ C44Þw;rz þ ðe15 þ e31Þφ;rz ¼ 0 C13 þ C44ð Þ 1 r ru;z À Á ;r þ C44 w;rr þ 1 r w;r þ C33w;zz þ e15 φ;rr þ 1 r φ;r þ e33φ;zz ¼ 0 e15 þ e31ð Þ 1 r ru;z À Á ;r þ e15 w;rr þ 1 r w;r þ e33w;zz À E11 φ;rr þ 1 r φ;r À E33φ;zz ¼ 0 (7.60) Equation (7.32) becomes σzðr; 0Þ ¼ ÀpðrÞ; Dzðr; 0Þ ¼ qðrÞ; when r a wðr; 0Þ ¼ φðr; 0Þ ¼ 0; when r a; τrz ¼ 0; À1 ðx1; x2Þ 1 (7.61) Introduce the Hankel transform pair withJk; Jk is the Bessel’s function of the ﬁrst kind of order k: Fðξ; zÞ ¼ Z 1 0 Fðr; zÞrJkðξrÞdr; Fðr; zÞ ¼ Z 1 0 Fðξ; zÞξJkðξrÞdξ (7.62) 352 7 Three-Dimensional and Applied Electroelastic Problems
15. 15. Applying the Hankel transform, Eq. (7,62) to Eq. (7,60) with k ¼ 1 for u and k ¼ 0 for w and φ yields C44 u00 À C11ξ2 u À ðC13 þ C44Þξ w0 À ðe15 þ e31Þξφ0 ¼ 0 ðC13 þ C44Þξu0 þ C33 w00 À C44ξ2 w þ e33 φ00 À e15ξ2 φ ¼ 0 ðe15 þ e31Þξu0 þ e33 w00 À e15ξ2 w À E33 φ00 þ E11ξ2 φ ¼ 0 (7.63) where a prime indicates the derivative with respect to z. The solutions are assumed in the forms uðξ; zÞ ¼ ^uðξÞeÀη ξ z ; wðξ; zÞ ¼ ^wðξÞeÀη ξ z ; φ ¼ ^φeÀη ξ z (7.64) Substituting Eq. (7,64) into Eq. (7,63) yields C44η2 À C11 ðC13 þ C44Þη ðe15 þ e31Þη ÀðC13 þ C44Þη C33η2 À C44 e33η2 À e15 Àðe15 þ e31Þη e33η2 À e15 ÀE33η2 þ E11 2 4 3 5 ^u ξð Þ ^w ξð Þ ^φ ξð Þ 8 : 9 = ; ¼ 0 0 0 8 : 9 = ; (7.65) In order to have nontrivial solutions for ^u; ^w and ^φ , it should obtain the characteristic equation η6 þ B1η4 þ B2η2 þ B3 ¼ 0 (7.66) where B1; B2 and B3 are coefﬁcients constituted of material constants. Since coefﬁcients in Eq. (7.66) are real, in general it has six roots. Because the upper half space (z ! 0) is discussed, without loss of generality, we take eigenvalue η1 is a real positive number and η2; η3 are, in general, a pair of complex conjugates with positive real part. One form of the corresponding eigenvectors is ^uiðξÞ ¼ αiηi ^wiðξÞ; αi ¼ ðe15 þ e31Þ C33η2 i À C44 À Á À e33η2 i À e15 À Á ðC13 þ C44Þ e33η2 i À e15 À Á C44η2 i À C11 À Á þ ðe15 þ e31ÞðC13 þ C44Þη2 i ^φiðξÞ ¼ γiηi ^wiðξÞ; γi ¼ À C44η2 i À C11 À Á α þ ðC13 þ C44Þ ðe15 þ e31Þηi ; i ¼ 1; 2; 3 (7.67) Let ^wiðξÞ ¼ ð1 ηiξ= ÞfiðξÞ. Through the inverse transform, the general solutions are uðr; zÞ ¼ X3 i¼1 αi Z 1 0 fiðξÞeÀηi ξ z J1ðξrÞdξ φðr; zÞ ¼ X3 i¼1 γi Z 1 0 fiðξÞeÀηi ξ z J0ðξrÞdξ wðr; zÞ ¼ X3 i¼1 ð1 ηi= Þ Z 1 0 fiðξÞeÀηi ξ z J0ðξrÞdξ (7.68) 7.2 A Penny-Shaped Crack in Transversely Isotropic Material 353
16. 16. Using relations J1ðξrÞ½ ;r ¼ ξ J0ðξrÞ À ð1 2= ÞJ1ðξrÞ½ ; J0ðξrÞ½ ;r ¼ ÀξJ1ðξrÞ, the generalized stresses are σzðr; zÞ ¼ X3 i¼1 C13αi À C33 À e33ηiγið Þ Z 1 0 ξfiðξÞeÀηi ξ z J0ðξrÞdξ τrzðr; zÞ ¼ X3 i¼1 ÀC44 ηi= À C44ηiαi À e15γið Þ Z 1 0 ξfiðξÞeÀηi ξ z J1ðξrÞdξ Dzðr; zÞ ¼ X3 i¼1 e31αi À e33 þ E33ηiγið Þ Z 1 0 ξfiðξÞeÀηi ξ z J0ðξrÞdξ (7.69) For discussed penny-shaped crack (Fig. 7.1), since τrz r; zð Þ0 ¼ 0 due to symmetry, Eq. (7.69) yields X3 i¼1 ÀC44 ηi= À C44ηiαi À e15γið Þfi ¼ 0 (7.70) Eliminating f3 from Eq. (7.68), (7.69), and (7.70) and then substituting the results into Eq. (7.61), two pairs of integral equations are obtained: Z 1 0 fiðξÞξJ0ðρξÞdξ ¼ ti1p þ ti2q; for ρ 1; ρ ¼ r a= Z 1 0 fiðξÞξJ0ðρξÞdξ ¼ 0; for ρ 1; i ¼ 1; 2 (7.71) where t11 ¼ k22a2 H= ; t12 ¼ Àk12a2 H= ; t21 ¼ Àk21a2 H= ; t22 ¼ k11a2 H= k11 ¼ C13α1 À C33 À γ1η1e33 þ Δ1 C13α3 À C33 À γ3η3e33ð Þ k12 ¼ C13α2 À C33 À γ2η2e33 þ Δ2 C13α3 À C33 À γ3η3e33ð Þ k21 ¼ e31α1 À e33 þ γ1η1 E33 þ Δ1 e13α3 À e33 þ γ3η3e33ð Þ k22 ¼ e31α2 À e33 þ γ2η2 E33 þ Δ2 e13α3 À e33 þ γ3η3e33ð Þ H ¼ k11k22 À k12k21; Δ1 ¼ À C44 1 η1 þ η1α1=ð Þ þ e15γ1 C44 1 η3 þ η3α3=ð Þ þ e15γ3 ; Δ2 ¼ À C44 1 η2 þ η2α2=ð Þ þ e15γ2 C44 1 η3 þ η3α3=ð Þ þ e15γ3 (7.72) The solution of the dual integral equations in Eq. (7.71) is fiðξÞ ¼ 2 π Z 1 0 μ sinðμξÞdμ Z 1 0 ρ ti1pðρÞ þ ti2qðρÞ½  ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 1 À ρ2 p dρ (7.73) 354 7 Three-Dimensional and Applied Electroelastic Problems
17. 17. When uniform pressure p0 is applied over the area of radius r ¼ c a and uniform charge q0 applied over the area of r ¼ b a, we get σz ρ; 0ð Þ ¼ À 2p0 πa 1 À ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 1 À c a=ð Þ2 q arcsin 1 ρ=ð Þ À 1 ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ρ2 À 1 p # ; ρ ! 1 Dz ρ; 0ð Þ ¼ À 2q0 πa 1 À ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 1 À b a=ð Þ2 q arcsin 1 ρ=ð Þ À 1 ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ρ2 À 1 p # ; ρ ! 1 (7.74) The solution for a point force À P0 and point charge Q0 acted at the crack center ðr ¼ 0Þ can be obtained by using the limiting procedure lim c!0 πc2 p0 ¼ P0 and lim b!0 πb2 q0 ¼ Q0. The generalized stress intensity factors for uniform loadings p0 and q0 applied over r ¼ a are the same as shown in Eq. (7.51). For the point loadings are KI ¼ P0 ðπaÞ= 3 2= ; KD ¼ Q0 ðπaÞ= 3 2= (7.75) A modiﬁed stress intensity factor KÃ I for a semicircular surface crack in a homogeneous isotropic elastic material given by Cherepanov (1979) is KÃ I ¼ κðθÞKI; κðθÞ ¼ 1 þ 0:2 ðπ À 2θÞ π=½  2 (7.76) In the Vicker’s indentation cracking of experiments, a semicircular surface crack is located in an isotropic plane ðx1; x2Þ, the stress intensity factor can approximately adopt Eq. (7.76), but it should take 2P0 instead of P0 in KI. There were many literatures discussing the penny-shaped crack, such as Ueda (2007) which discussed a penny-shaped crack in a functionally graded piezoelectric strip under thermal loading. 7.3 Ellipsoidal Inclusion and Inhomogeneity 7.3.1 Basic Concept of Electroelastic Green Functions A subdomain with prescribed eigenstrain in a matrix is usually called the inclusion, and material properties of the inclusion are the same with the matrix. A subdomain with different material properties from the matrix is usually called the inhomogene- ity. The eigenstrain may be introduced by many physical phenomena, such as phase transformation strains, thermal strains, and plastic strains. The eigenstrain will produce self-equilibrium stresses in a constrained matrix. Eshelby’s theory (1957) 7.3 Ellipsoidal Inclusion and Inhomogeneity 355
18. 18. of the inclusion and inhomogeneity problems is important in the analyses of piezoelectric composite materials. For convenience the notations given in Eq. (3.8) in Sect. 3.1 are adopted. A subscript in upper case takes the value 1,2,3, and 4 and a subscript in lower case takes the value 1,2, and 3. Figure 7.2 shows an ellipsoid inclusion occupied region Ωin in a 3D space R3 . In Ωin there is generalized eigenstrain ZÃ Zij ¼ εÃ ij; Z4j ¼ ÀEÃ j ; i; j ¼ 1; 2; 3; without Z44Þ. The constitutive equations with eigenstrain are ΣiJ ¼ EiJKlðZKl À ZÃ KlÞ; ZÃ KlðxÞ ¼ ZÃ Kl; x 2 Ω; ZÃ KlðxÞ ¼ 0; x =2 Ω (7.77) where ZKl ¼ UK;l; U ¼ uk; φ½ T . The generalized equilibrium equations are ΣiJ;i ¼ ÀfJ; EiJKlUK;li ¼ EiJKlZÃ Kl;i xð Þ À fJ (7.78) where f1; f2; f3 are components of the body force and f4 ¼ Àρe is the body electric charge density. From Eq. (7.78), it is seen that the role of EiJKlZÃ Kl;iðxÞ is analogous to the body force. The Green function GKR;ilðx À x0 Þ in an inﬁnite body is deﬁned as EiJKlGKR;ilðx À x0 Þ þ δJRδðx À x0 Þ ¼ 0 (7.79) where δJR is the generalized Kronecker delta and δðx À x0 Þ is the three-dimensional Dirac delta function. Except x ¼ x0 ; δðx À x0 Þ ¼ 0, and for a regular function fðxÞ, Z 1 À1 fðx0 Þδðx À x0 Þdx0 ¼ fðxÞ (7.80) The Green function deﬁned in Eq. (7.79) satisﬁes the generalized equilibrium equation. GIJðx À x0 Þ and its derivative approach zero when x À x0 j j ! 1. The electroelastic Green function GIJðx À x0 Þ is extensively applied to study the inclusion and inhomogeneity problems in piezoelectric materials. Gijðx À x0 Þ denotes the elastic displacement at x in the xi direction due to a unit point force at x0 in the xj direction; Gi4ðx À x0 Þ denotes the elastic displacement at x in the xi direction due to a unit point charge at x0 ; G4jðx À x0 Þ denotes the electric potential at xdue to a unit point force atx0 in thexj direction; andG44ðx À x0 Þdenotes the electric potential at x due to a unit point charge at x0 . Fig. 7.2 An elliptic inclusion 356 7 Three-Dimensional and Applied Electroelastic Problems
19. 19. 7.3.2 Fourier Transform Method Assume that the generalized eigenstrains and displacements can be expressed as (Mura 1987) ZÃ KlðxÞ ¼ ZÃ KlðξÞeiξÁx ; UKðxÞ ¼ UKðξÞeiξÁx (7.81) Analogous to elasticity, substituting Eq. (7.81) into (7.78) and neglecting the body force yield ΠJKðξÞ UK ¼ ΞJðξÞ;; ΠJKðξÞ ¼ EiJKlξiξl; ΞJðξÞ ¼ ÀiEiJKl ZÃ Klξi UK ¼ ΞJNJK D= ; NMJðξÞ ¼ 1 2 ϖIKLϖJMNΠKMΠLN; D ¼ ΠKMj j (7.82) where ϖJMN is the permutation tensor and NMJ is the algebraic complement of ΠMJ in the matrix Π. For the general case, the Fourier integral transform is used (Mura 1987; Wang 1992): ZÃ KlðxÞ ¼ Z 1 À1 ZÃ KlðξÞ eiξÁx dξ; ZÃ Kl ξð Þ ¼ 1 2π3 Z 1 À1 ZÃ KlðxÞ eÀiξÁx dx UKðxÞ ¼ Z 1 À1 UKðξÞ eiξÁx dξ; UK ξð Þ ¼ 1 2π3 Z 1 À1 UKðxÞ eÀiξÁx dx (7.83) Analogous to elasticity, substituting Eq. (7.83) into (7.78) and using (7.82) yield UMðxÞ ¼ Ài Z 1 À1 EiJKl ZÃ KlðξÞξiNMJðξÞDÀ1 ðξÞ eiξÁx dξ or UMðxÞ ¼ À Z 1 À1 EiJKlZÃ Klðx0 ÞGMJ;iðx À x0 Þdx0 GMJðx À x0 Þ ¼ 1 2π3 Z 1 À1 NMJðξÞDÀ1 ðξÞ eiξÁ xÀx0 ð Þ dξ (7.84) where GMJ;iðx À x0 Þ ¼ @GMJðx À x0 Þ @xi= ¼ À@GMJðx À x0 Þ @x0 i . If GMJðx À x0 Þ is a Green function in a ﬁnite region, then UMðxÞ ¼ Z a EiJKlZÃ Klðx0 ÞniGMJðx À x0 Þda x0 ð Þ À Z V EiJKlZÃ Kl;iðx0 ÞGMJðx À x0 ÞdVðx0 Þ (7.85) 7.3.3 Radon Transform Method The Radon integral transform plays a fundamental role in the tomography, such as CT scanning in medicine. At ﬁrst the basic concepts are introduced as follows (Deans 1983): An arbitrary function fðx1; x2Þ is deﬁned on some domain Ω of a 2D plane R2 . Let L be any line in the plane, then the mapping deﬁned by the projection or line integral of f along all possible lines L is the 2D Radon transform of f, i.e., 7.3 Ellipsoidal Inclusion and Inhomogeneity 357
20. 20. fðω; ϕÞ ¼ Rf ¼ Z L fðx1; x2Þ ds ¼ Z 1 À1 fðωξ þ τηÞdτ; or fðω; ξÞ ¼ Z R2 fðxÞδ ω À ξ Á xð Þ daðxÞ (7.86) where ω ¼ ξ Á x ¼ x1 cos ϕ þ x2 sin ϕ is the perpendicular distance from the origin to L, ξ ¼ cos ϕ; sin ϕð Þ is a unit vector along ω which deﬁnes the orientation of L, η ¼ ðÀ sin ϕ; cos ϕÞ?ξ is along L, τ is determined by x ¼ ωξ þ τη, and ϕ is the angle between ξ and positive x1-axis (Fig. 7.3). The last equation in Eq. (7.86) is easy extended to three- and higher-dimensional space. If fðω; ξÞ is known for all ω and ϕ, then fðω; ξÞis a 2D Radon transform of f ðx1; x2Þ. In an n-dimensional space, L represents ðn À 1Þ-dimensional hyperplane. Especially for a 3D space, L repre- sents a plane. For n-dimensional space, the inversion Radon transform is fðxÞ ¼ 1 2ð2πiÞnÀ1 ΔðnÀ1Þ 2= x Z ξj j¼1 Rfðξ; ξ Á xÞdaðξÞ (7.87) whereΔx is the Laplacian operator. Especially for 3D space, Eq. (7.87) is reduced to fðxÞ ¼ À 1 8π2 Δ3 Z ξj j¼1 Rfðξ; ξ Á xÞdξ ¼ À 1 8π2 Z ξj j¼1 @2 fðξ; ξ Á xÞ @ω2 Â Ã ω¼ξÁx daðξÞ (7.88) Deeg (1980), Dunn and Taya (1993), and Dunn (1994) pointed out that the Radon transform can also be used to the electroelastic Green function GIJðx À x0 Þ, i.e., GIJðξ; ω À ξ Á x0 Þ ¼ ð ð ξÁx¼ω GIJðx À x0 ÞdaðxÞ GIJðx À x0 Þ ¼ 1 8π2 ð ð ξj j¼1 @2 GIJðξ; ω À ξ Á x0 Þ @ω2 Â Ã ξÁx¼ω daðξÞ (7.89) Fig. 7.3 A sketch of Radon transform 358 7 Three-Dimensional and Applied Electroelastic Problems
21. 21. whereξ; ωare variables in the transform space and the integral domain is a 2D plane ξ Á x ¼ ω. In the inverse Radon transform, the integral domain is the surface of a unit sphere ξj j ¼ 1. Using the Radon transform to Eq. (7.79), after some mani- pulation, yields KJMðξÞð@2 @xk@xk= Þ GMRðξ; ω À ξ Á x0 Þ þ δJRδðω À ξ Á x0 Þ ¼ 0 (7.90) where KJMðξÞ ¼ EiJMnξiξn . Using the inversion Radon transform from Eq. (7.90) yields GMRðx À x0 Þ ¼ 1 8π2 x À x0j j ð ð ξj j¼1 KÀ1 MRðξÞδðξ Á tÞdaðξÞ (7.91) where KJMðξÞKÀ1 MRðξÞ ¼ δJR and t is the unit vector along x À x0 . Using the property of the Dirac delta, in an orthogonal coordinate system t-m-n, Deeg (1980) reduced the integral in Eq. (7.91) to the following contour integral: GMRðx À x0 Þ ¼ 1 8π2 x À x0j j Z C KÀ1 MRðξÞδðξ Á tÞdaðξÞ (7.92) where C is the contour produced by ξj j ¼ 1 in m-n plane normal to x À x0 . Compared to Fourier transform method, Eq. (7.92) is a simpler effective method to seek the Green function. The second partial derivatives of the electroelastic Green function is GMR;klðx À x0 Þ ¼ 1 8π2 x À x0j j @2 @xn@xn Z ξj j¼1 ξkξlKÀ1 MRðξÞδ ξ Á ðx À x0 Þ½ daðξÞ (7.93) 7.3.4 A Single Ellipsoidal Inclusion with Uniform Eigenstrains Let the coordinates coincide with the principle axes of the material. For an ellipsoidal inclusion with uniform eigenstrains, the Eshelby’s method is used. At ﬁrst the inclusion is cut off from the matrix, so the inclusion and matrix are all free. The eigenstrains of the inclusion in the free state is denoted by ZÃ . The following generalized stresses are applied on the boundary of the inclusion: TJ ¼ ÀΣÃ iJ Á ni; ΣÃ iJ ¼ EiJMlZÃ Ml (7.94) Then put the inclusion subjected to above generalized stresses into the matrix. After this procedure, the original problem is transformed to a homogeneous 7.3 Ellipsoidal Inclusion and Inhomogeneity 359
22. 22. material with a force À TJ ¼ EiJMlZÃ Ml acting on the counter which originally is the boundary of the inclusion. If ZÃ is uniform, Eq. (7.94) yields (Deeg 1980) UM;nðξÞ ¼ ÀEiJKlZÃ Kl ð ð ð Ω GMJ;inðx À x0 ÞdVðx0 Þ (7.95) Using Eq. (7.93) from Eq. (7.95) yields (Deeg 1980; Dunn and Taya 1993) UM;nðξÞ ¼ a1a2a3 4π EiJKlZÃ Kl Z ξj j¼1 1 α3 ξkξlKÀ1 MRðξÞdaðξÞ; α ¼ ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ a2 1ξ2 1 þ a2 2ξ2 2 þ a2 3ξ2 3 q (7.96) Analogous to the elastic inclusion problem, the generalized strains inside the ellipsoid induced by the uniform eigenstrains are also uniform and ZMnðξÞ ¼ SMnKlZÃ Kl SMnKl ¼ ð1 8π= ÞEiJKl IMJin þ InJiMð Þ; M ¼ 1; 2; 3 ð1 4π= ÞEiJKlI4Jin; M ¼ 4 IMJin ¼ a1a2a3 Z ξj j¼1 1 α3 À Á GMJin ξð Þda ξð Þ; GMJinðξÞ ¼ ξiξnKÀ1 MJðξÞ (7.97) where SMnKl is called the “electroelastic Eshelby tensor,” but it is not a tensor, i.e., it does not obey the tensor transform rule under a coordinate transformation. The key point to solve SMnKl is to calculate IMJinðξÞ. IMJinðξÞ can be transformed to the following form (Mikata 2000): IMJinðξÞ ¼ Z ξj j¼1 GMJin y1 a1= ; y2 a12= ; y3 a3=ð ÞdaðξÞ ¼ Z 1 À1 dt Z 2π 0 GMJin y1 a1= ; y2 a12= ; y3 a3=ð Þdϕ y1 ¼ ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 1 À t2 p cos ϕ; y2 ¼ ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 1 À t2 p sin ϕ; y3 ¼ t (7.98) For transversely isotropic piezoelectric materials, Mikata (2000) pointed out that in IMJin ξð Þ only I1212; I1313; I1314; I2323; I2324 and I11MJ; I22MJ; I33MJ; MJ ¼ 11; 22; 33; 44; 34 are not zero, and the Eshelby tensor only has 36 components: S1111; S1122; S1133; S1143; S1212 ¼ S1221 ¼ S2112 ¼ S2121; S1313 ¼ S1331 ¼ S3113 ¼ S3131; S1341 ¼ S3141; S2211; S2222; S2233; S2243; S2323 ¼ S2332 ¼ S3223 ¼ S3232; S2342 ¼ S3242; S3311; S3322; S3333; S3343; S4113; S4141; S4223; S4242; S4311; S4322; S4333; S4343: For an elliptic cylindrical inclusion along the x3-axis, the Eshelby tensor with 22 components is 360 7 Three-Dimensional and Applied Electroelastic Problems
23. 23. S1111 ¼ α 2ð1 þ αÞ2 3 þ C12 C11 þ 2 α ; S1122 ¼ α 2ð1 þ αÞ2 ð2 þ αÞC12 αC11 þ 2 α ! À 1; S1133 ¼ C13 ð1 þ αÞC11 ; S1143 ¼ e31 ð1 þ αÞC11 ; S1212 ¼ α 2ð1 þ αÞ2 1 þ α þ α2 α À C12 C11 ; S1313 ¼ 1 2ð1 þ αÞ ; S2233 ¼ αC13 ð1 þ αÞC11 ; S2243 ¼ αe13 ð1 þ αÞC11 ; S2323 ¼ α 2ð1 þ αÞ ; S2211 ¼ α 2ð1 þ αÞ2 ð1 þ 2αÞ C12 C11 À 1 ! ; S2222 ¼ α 2ð1 þ αÞ2 3 þ C12 C11 þ 2α ; S4141 ¼ 1 ð1 þ αÞ ; S4242 ¼ α ð1 þ αÞ ; other SMnKl ¼ 0 S1212 ¼ S1221 ¼ S2112 ¼ S2121; S1313 ¼ S1331 ¼ S3113 ¼ S3131; S2323 ¼ S2332 ¼ S3223 ¼ S3232 (7.99a) For a penny-shaped crack perpendicular to x3 -axis, the Eshelby tensor with 18 components is S1313 ¼ S1331 ¼ S3113 ¼ S3131 ¼ S2323 ¼ S2332 ¼ S3223 ¼ S3232 ¼ 1 2= S1341 ¼ S3141 ¼ S2342 ¼ S3242 ¼ e15 2C44 ; S3311 ¼ S3322 ¼ C13 E33 þ e31e33 C33 E33 þ e2 33 S3333 ¼ S4343 ¼ 1; S4311 ¼ S4322 ¼ C13e33 À C33e31 C33 E33 þ e2 33 ; other SMJin ¼ 0 (7.99b) 7.3.5 Ellipsoid Inhomogeneity Analogous to elastic inhomogeneity problem, the electroelastic inhomogeneity prob- lem can be handled by the equivalent inclusion method. Let EM iJKl and Ein iJKl denote the material constants in the matrix and inhomogeneity, respectively. The generalized stress Σ0 Mn is applied at inﬁnity. Obviously for a homogeneous material, the generalized stress in material is also Σ0 Mn and the corresponding strain is Z0 Mn ¼ EM iJMn À ÁÀ1 Σ0 Mn. Assume the strain due to the inhomogeneity is ZMn and then the stress in the matrix and inhomogeneity are, respectively, ΣM iJ ðxÞ ¼ EM iJMn Z0 Mn þ ZMn xð Þ Â Ã ; Σin iJðxÞ ¼ Ein iJMn Z0 Mn þ ZMnðxÞ Â Ã (7.100) The key point of the equivalent inclusion method is that let the inhomogeneity possess the same material constants with the matrix, but the artiﬁcial eigenstrain ZÃ Mn is added. Then let Σin iJðxÞ ¼ Ein iJMn Z0 Mn þ ZMnðxÞ Â Ã ¼ EM iJMn Z0 Mn þ ZMnðxÞ þ ZÃ Mn Â Ã (7.101) 7.3 Ellipsoidal Inclusion and Inhomogeneity 361
24. 24. Using ZMnðxÞ ¼ SMnKlZÃ Kl in the inhomogeneity, so Eq. (7.101) yields ZÃ Kl ¼ EM iJMn À Ein iJMn À Á SMnKl þ EM iJKl Â ÃÀ1 Ein iJMn À EM iJMn À Á Z0 Mn (7.102) Solving ZÃ Kl, the problem can be solved. As an example an ellipsoidal piezoelectric sensor embedded in an elastic material is discussed (Fan and Qin 1995). The constitutive equations of the sensor (as an elliptic inclusion) and matrix are, respectively, σij ¼ Cin ijklεkl À ein kijEk; Di ¼ ein iklεkl þ Ein ikEk; in Ωin (7.103) σij ¼ CM ijklεkl; Di ¼ EM ik Ek; in ΩM (7.104) Comparing Eqs. (7.103) and (7.104), one can consider the terms ein kijEk; ein iklεkl in Eq. (7.103) produced by some kind of eigenstrains. When the matrix is subjected to uniform generalized stresses σ0 ij; E0 i at inﬁnity, the generalized stresses in the sensor are changed to σin ij ¼ σ0 ij þ σ0in ij ¼ Cin ijkl ε0 kl þ εkl À εE kl À Á ; Cin ijklεE kl ¼ ein kij Ek þ E0 k À Á (7.105) Din i ¼ D0 i þ D0in i ¼ Ein ik E0 k þ Ek À Eε k À Á ; ÀEin ikEε k ¼ ein ikl εkl þ ε0 kl À Á (7.106) By using the equivalent inclusion method, the original inhomogeneity problem subjected to uniform generalized stresses at inﬁnity can be decoupled into two equivalent inclusion problems: 1. The elastic equivalent inclusion problem. Equation (7.105) can also be written as σin ij ¼ σ0 ij þ σ0in ij ¼ CM ijkl ε0 kl þ εkl À εE kl À εÃ kl À Á (7.107) where εÃ kl is the virtual eigenstrain. Using the Eshelby inclusion theory yields εkl ¼ SklmnεÃÃ kl ; εÃÃ kl ¼ εE kl þ εÃ kl (7.108) 2. The dielectric equivalent inclusion problem. Equation (7.106) can also be written as Din i ¼ D0 i þ D0in i ¼ EM ik E0 k þ Ek À Eε k À EÃ k À Á (7.109) where EÃ k is the virtual eigen electric ﬁeld. Using the Eshelby inclusion theory yields Ek ¼ sklEÃÃ l ; EÃÃ k ¼ Eε k þ EÃ k (7.110) 362 7 Three-Dimensional and Applied Electroelastic Problems
25. 25. where skl ¼ S4k4l. Comparing Eqs. (7.105) and (7.107), it is concluded that CM ijkl ε0 kl þ SklmnεÃÃ kl À εÃÃ kl À Á ¼ Cin ijkl ε0 kl þ SklmnεÃÃ kl À εE kl À Á ¼ Cin ijkl ε0 kl þ SklmnεÃÃ kl À Á À ein kij sklEÃÃ l þ E0 k À Á (7.111) Comparing Eqs. (7.106) and (7.110), it is concluded that Ein ik E0 k þ sklEÃÃ l À Eε k À Á ¼ EM ik E0 k þ sklEÃÃ l À EÃÃ k À Á ; or EÃÃ l ¼ sml EM im À Ein im À Á À EM ik Â ÃÀ1 Ein im À EM im À Á E0 k þ ein imnSmnpqεÃÃ pq þ ein iklε0 kl h i (7.112) Solving εÃÃ kl and EÃÃ k , the stress and electric ﬁelds are obtained in the sensor, i.e., σin ij ¼ CM ijkl ε0 kl þ SklmnεÃÃ kl À εÃÃ kl À Á ¼ Cin ijkl ε0 kl þ SklmnεÃÃ kl À Á À ein kij sklEÃÃ l þ E0 k À Á Din i ¼ EM ik E0 k þ sklEÃÃ l À EÃÃ k À Á ¼ Ein ik E0 k þ sklEÃÃ l À Eε k À Á (7.113) The stress σout ij and electric ﬁelds Eout in the matrix can be solved as follows: σout ij ¼ σ0 ij þ σ0out ij ¼ σ0 ij þ ½½σij þ σ0in ij ; ½½σij ¼ σ0out ij À σ0in ij ¼ σout ij À σin ij Eout i ¼ E0 i þ E0out i ¼ E0 i þ ½Ei½  þ E0in i ; ½Ei½  ¼ E0out i À E0in i ¼ Eout i À Ein i (7.114) The displacement u and the surface traction σ Á n ¼ 0 across the interface of inclusion and matrix must be continuous, and jump of the displacement gradient r u must be normal to the interface. The continuous conditions of the electric ﬁeld and electric displacement E Â n and D Á n across the interface demand that the jump of E must be normal to the interface. So ½ui½  ¼ uout i À uin i ¼ 0; ½½ui;j ¼ uout i;j À uin i;j ¼ λinj; ½½σijnj ¼ 0 ½Ei½  ¼ ηni; ½Di½ ni ¼ 0 (7.115) where λ; η are proportional constants. Substituting the constitutive equations into Eq. (7.115), it is obtained: Cijklλknlnj ¼ ÀCijklεÃÃ kl nj; ηEiknink ¼ ÀEikniEÃÃ k (7.116) Therefore, the stress σout ij and electric ﬁelds Eout in the matrix are σout ij ¼ σ0 ij þ Cijkl λknl þ εÃÃ kl À Á þ σ0in ij ; Eout i ¼ E0 i þ Eik ηnk þ EÃÃ k À Á þ E0in i (7.117) 7.3 Ellipsoidal Inclusion and Inhomogeneity 363
26. 26. 7.4 Some Simpler Practical Problems 7.4.1 Extension of a Rod Figure 7.4 shows a transversely isotropic piezoelectric long cylindrical rod with polarized x3 -axis. The two silver-coated end faces are used as electrodes and subjected to uniform normal traction p. Using the ﬁrst kind of constitutive equation, the solutions of this problem are as follows: 1. For shorted electrodes, σ33 ¼ p; all other σij ¼ 0; ε33 ¼ s33p; ε11 ¼ ε22 ¼ s13p; E3 ¼ E1 ¼ E2 ¼ 0; D3 ¼ d33p; D1 ¼ D2 ¼ 0; As ¼ σ33ε33 2= ¼ s33p2 2= (7.118) 2. For open electrodes, σ33 ¼ p; all other σij ¼ 0; ε33 ¼ s33 1 À d2 33 E33s33= À Á p; ε11 ¼ ε22 ¼ s13p þ d31E3; D3 ¼ D1 ¼ D2 ¼ 0; E3 ¼ À d33 E33=ð Þp; E1 ¼ E2 ¼ 0; Uo ¼ s33 2=ð Þ 1 À d2 33 E33s33= À Á p2 (7.119) The rod appears to be stiffer for the open electrodes than sorted electrodes due to d2 33 E33s33= 0. 3. The longitudinal electromechanical coupling factor k33: k2 33 ¼ ðUs À UoÞ Us= ¼ d2 33 E33s33= (7.120) 7.4.2 Torsion of a Piezoelectric Circular Cylinder Figure 7.5 shows a transversely isotropic piezoelectric circular cylinder of length L, inner radius a, and outer radius b with polarized θ-axis. The two silver-coated end faces are used as electrodes and subjected to a torque M and charge Qe. Using the second kind of constitutive equation, the general solution of this problem is Fig. 7.4 An axial poled rod 364 7 Three-Dimensional and Applied Electroelastic Problems
27. 27. uθ ¼ Arz; ur ¼ uz ¼ 0; γθz ¼ Ar; σθz ¼ C44Ar À e15B; φ ¼ ÀBz; Ez ¼ B; Dz ¼ e15Ar þ E11B M ¼ Z b a σθzð2πrdrÞr ¼ C44AIp À e152πB b3 À a3 À Á 3= ; Ip ¼ π b4 À a4 À Á 2= Qe ¼ Z b a Dzð2πrdrÞ ¼ e152πA b3 À a3 À Á 3= þ E11Bπ b2 À a2 À Á (7.121) 1. Shorted electrodes : B ¼ 0; A ¼ M C44= Ip (7.122) 2. Open electrodes : Qe ¼ 0; A ¼ M C44Ip þ e2 15 E11 2π 3 2 b3 À a3 ð Þ π b2 À a2ð Þ #À1 (7.123) 7.4.3 A Circular Hole Under Longitudinal Shear in an Inﬁnite Piezoelectric Plate Figure 7.6 shows a circular cylindrical hole of radius R in an unbounded transversely isotropic piezoelectric material with polarized x3-axis under a uniform longitudinal shear stress σ23 ¼ τ0 at x2 ¼ Æ1. The hole surface is a grounded electrode. The governing equations and boundary conditions for an electrically open case are r2 u3 ¼ 0; r2 φ ¼ 0; r R σrz ¼ 0; φ ¼ 0; r ¼ R; σ23 ¼ τ0; x2 ¼ Æ1 D2 ¼ 0; x2 ¼ Æ1 ðelectrically openÞ; E2 ¼ 0; x2 ¼ Æ1 ðelectrically shortedÞ (7.124) Fig. 7.5 A circular cylinder in torsion Fig. 7.6 An inﬁnite plate with a circular cylindrical hole under longitudinal shear 7.4 Some Simpler Practical Problems 365
28. 28. For the electrically open case, the solution is u3 ¼ τ0 C44 1 þ k2ð Þ r þ 1 þ 2 k2 À Á R2 r ! sin θ; φ ¼ τ0 C44E11 1 þ k2ð Þ r À R2 r sin θ (7.125) where k2 ¼ e2 15 C44E11= . For the electrically shorted case, the solution can also be obtained. 7.4.4 Thickness-Shear Vibration of a Quartz Plate Figure 7.7 shows the sketch of a widely used piezoelectric resonator manufactured by rotated Y-cut quartz plate. Surfaces at x2 ¼ Æh are traction-free and electroded, with a driving voltage V0eiωt . Let u3 ¼ 0 and @u2 @x2= % 0 due to the plate is thin enough. So the displacement and potential ﬁelds can be assumed in the following forms: u1 ¼ U1ðx2Þeiωt ; u2ðx2Þ % 0; u3 ¼ 0; φ ¼ Φðx2Þeiωt (7.126) Under above assumptions, the constitutive equations are σ6 ¼ C66u1;2 þ e26φ;2; D2 ¼ e26u1;2 À E22φ;2 (7.127) The stresses σ5 ¼ C56u1;2 þ e25φ;2; D3 ¼ e36u1;2 À E23φ;2 are omitted because they are not used. The generalized momentum equation and boundary condition are σ6;2 ¼ Àρω2 u1; D2;2 ¼ 0 σ6 ¼ 0; at x2 ¼ Æh; ΦðhÞ À ΦðÀhÞ ¼ V0 (7.128) The general solutions are U1 ¼ A1 sin λx2 þ A2 cos λx2; λ ¼ ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ρ CÃ 66 q ω; CÃ 66 ¼ C66 1 þ k2 À Á ; k ¼ e26 ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ C66E22 p. Φ ¼ ðe26 E22= Þ A1 sin λx2 þ A2 cos λx2ð Þ þ Bx2 (7.129) Fig. 7.7 An electrode quartz plate 366 7 Three-Dimensional and Applied Electroelastic Problems
29. 29. From the boundary conditions, we can get two group equations: CÃ 66A1λ cos λh þ e26B ¼ 0; 2 e26 E22=ð ÞA1 sin λh þ 2Bh ¼ V0 (7.130) CÃ 66A2λ sin λh ¼ 0 (7.131) 1. Free vibration V0 ¼ 0, symmetric modes From Eq. (7.131) it is obtained sin λh ¼ 0; or λnh ¼ nπ 2= ; ωn ¼ ðnπ 2h= Þ ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ CÃ 66 ρ= q ; n ¼ 0; 2; 4; 6; . . . ; (7.132) whereωn is the nth order resonance frequency. In the same timeA2 6¼ 0; A1 ¼ B ¼ 0. The corresponding symmetric modes are U1 ¼ cos λnx2; Φ ¼ ðe26 E22= Þ cos λnx2 (7.133) 2. Free vibrationV0 ¼ 0, antisymmetric modes In this caseA1 6¼ 0; B 6¼ 0; A2 ¼ 0. Nontrivial solutions may exist in Eq. (7.130) if CÃ 66A1λh cos λh À e2 26 E22= À Á sin λh ¼ 0; or tan λνh ¼ λνhð1 þ k2 Þ k2 ; ων ¼ λν ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ CÃ 66 ρ= q (7.134) From Eq. (7.130), it is obtained Bν ¼ À CÃ 66 e26= À Á A1λν cos λνh. In this case sin λh 6¼ 0, so A2 ¼ 0. The corresponding antisymmetric modes are U1 ¼ sin λx2; Φ ¼ e26 E22=ð Þ sin λx2 À CÃ 66 e26= À Á λν cos λνh Â Ã x2 (7.135) 3. Forced vibration From Eq. (7.131) we have A2 ¼ 0. From Eq. (7.130) we get A1 ¼ À V0 2 e26V0 CÃ 66λh cos λh À e2 26 E22= À Á sin λh ; B ¼ V0 2 CÃ 66λ cos λh CÃ 66λh cos λh À e2 26 E22= À Á sin λh (7.136) Yang (2005) gave also some other interest problems except the above examples in this section. 7.5 Laminated Piezoelectric Plates 7.5.1 Basic Concepts and Governing Equations In the earlier work, the piezoelectric actuator structure constituted of an elastic substrate (beam or bar), electroded piezoelectric elements, and ﬁnite-thickness bonding layers. For a pair actuators ﬁxed on the upper and lower surfaces, if the 7.5 Laminated Piezoelectric Plates 367
30. 30. same voltage is applied to both actuators, it results in pure extension, and if the opposite voltage is applied to both actuators, it results in bending (Fig. 7.8). In the present time, the “intelligent structure” may be a laminated piezoelectric beam, plate, shell and distributed actuator, sensor, and processor networks. In engineering the classical beam, plate and shell theory are commonly used, and sometimes will use the higher-order theories. Consider anN-layer laminated piezoelectric plate of dimensionsL1 andL2 inx1 and x2 directions and total thickness H in x3-direction, and the ith layer has thickness hi. The plate is polarized along x3-axis. Except the global coordinate system, a local coordinate system x1; x2; zið Þ in the middle plane of ith layer is also adopted (Fig. 7.9). Layer 1 is the bottom layer and the layer N is the top layer. At each interface with perfect bonding between layers, continuity conditions of generalize displacements and tractions must be satisﬁed. For the ith interface between ith and ði þ 1Þth layers in the local coordinate system, the continuity conditions are UðiÞ x1; x2; hi 2=ð Þ ¼ Uðiþ1Þ x1; x2; Àhiþ1 2=ð Þ; ΣðiÞ nðiÞ x1; x2; hi 2=ð Þ ¼ Σðiþ1Þ nðiÞ x1; x2; Àhiþ1 2=ð Þ; i ¼ 1 À ðN À 1Þ (7.137) It is also noted that sometimes a bond-line may be simulated by a layer of small thickness. For each interface, there are eight continuity conditions, so for a laminate Fig. 7.8 A sketch of a simple intelligent beam Fig. 7.9 A multiply laminated piezoelectric plate 368 7 Three-Dimensional and Applied Electroelastic Problems
31. 31. plate with N layers, there are 8ðN À 1Þ continuity conditions; on the lower surface ðz ¼ Àh1 2= Þ of the ﬁrst layer and on the upper surface ðz ¼ hN 2= Þ of the Nth layer, there are four boundary conditions, respectively. Therefore, there are total 8N boundary conditions to determine 8N unknowns. For an orthotropic material layer, the constitutive equation is shown in Eq. (3.69). Analogous to Eq. (7.3), the motion equations in terms of generalized displacements are C11u1;11 þ C66u1;22 þ C55u1;33 þ ðC12 þ C66Þu2;12 þ ðC13 þ C55Þu3;13 þ ðe15 þ e31Þφ;13 ¼ ρu1;tt ðC12 þ C66Þu1;12 þ C66u2;11 þ C22u2;22 þ C44u2;33 þ ðC23 þ C44Þu3;23 þ ðe24 þ e32Þφ;23 ¼ ρu2;tt ðC13 þ C55Þu1;13 þ ðC23 þ C44Þu2;23 þ C55u3;11 þ C44u3;22 þ C33u3;33 þ e24φ;22 þ e33φ;33 ¼ ρu3;tt ðe31 þ e15Þu1;13 þ ðe32 þ e24Þu2;23 þ e15u3;11 þ e24u3;22 þ e33u3;33 À E11φ;11 À E22φ;22 À E33φ;33 ¼ 0 (7.138) 7.5.2 Bending in Simply Supported Orthotropic Laminated Rectangular Plate It is assumed that the bottom and lateral surfaces are free, and known normal traction and potential are imposed on the top surface: qðx1; x2Þ ¼ q0 sin p1x1 sin p2x2; φðx1; x2Þ ¼ Φ0 sin p1x1 sin p2x2 p1 ¼ ðnπ L1= Þ; p2 ¼ ðmπ L2= Þ; when x3 ¼ H (7.139) For the simply supported orthotropic laminated rectangular plate, the solution in each layer is assumed (Heyliger 1997): u1 ¼ u10esx3 cos p1x1 sin p2x2; u2 ¼ u20esx3 sin p1x1 cos p2x2 u3 ¼ u30esx3 sin p1x1 sin p2x2; φ ¼ φ0esx3 sin p1x1 sin p2x2 (7.140) where ui0; φ0; s are undetermined constants and the superscript (i) is omitted. Substituting Eq. (7.140) into (7.138) yields ΛU0 ¼ 0; U0 ¼ u10; u20; u30; φ0½ T ; Λ ¼ C11p2 1 þ C66p2 2 À C55s2 ðC12 þ C66Þp1p2 À ðC13 þ C55Þp1s À ðe15 þ e31Þp1s ðC12 þ C66Þp1p2 C66p2 1 þ C22p2 2 À C44s2 À ðC23 þ C44Þp2s À ðe24 þ e32Þp2s ðC13 þ C55Þp1s ðC23 þ C44Þp2s C55p2 1 þ C44p2 2 À C33s2 e15p2 1 þ e24p2 2 À e33s2 ðe15 þ e31Þp1s ðe24 þ e32Þp2s e15p2 1 þ e24p2 2 À e33s2 À E11p2 1 À E22p2 2 þ E33s2 2 6 6 6 6 6 6 4 3 7 7 7 7 7 7 5 (7.141) Equation (7.141) will have nontrivial solution if Λj j ¼ 0. From which we can obtained eight eigenvector si, si; i ¼ 1 À 8. Corresponding each si, an eigenvector 7.5 Laminated Piezoelectric Plates 369
32. 32. U0j (u10i; u20i; u30i; φ0i) with one unknown u10j is obtained. As shown in Sect. 7.5.1, the problem can be solved uniquely. 7.5.3 Free Vibration of Laminates in Cylindrical Bending Let L1 ! 1 in x1 direction and all variables be independent with x1 . Assuming u1 ¼ 0, from Eq. (7.138), the generalized motion equations are C22u2;22 þ C44u2;33 þ ðC23 þ C44Þu3;23 þ ðe24 þ e32Þφ;23 ¼ ρu2;tt ðC23 þ C44Þu2;23 þ C44u3;22 þ C33u3;33 þ e24φ;22 þ e33φ;33 ¼ ρu3;tt ðe32 þ e24Þu2;23 þ e24u3;22 þ e33u3;33 À E22φ;22 À E33φ;33 ¼ 0 (7.142) The continuity conditions on interface are shown in Eq. (7.137). For the free vibration, the mechanical boundary conditions on the top and bottom surfaces are σ33ðx2; hN 2= Þ ¼ σ33ðx2; Àh1 2= Þ ¼ σ23ðx2; hN 2= Þ ¼ σ23ðx2; Àh1 2= Þ ¼ 0 (7.143) The electrical boundary conditions have two different kinds: ð1Þ φ x2; hN 2=ð Þ ¼ φ x2; Àh1 2=ð Þ ¼ 0; or ð2Þ D3 x2; hN 2=ð Þ ¼ D3 x2; Àh1 2=ð Þ ¼ 0 (7.144) For the cylindrical bending vibration in ðx2; x3Þ plane, the boundary conditions on the lateral surfaces are σ22ð0; x3Þ ¼ σ22ð0; L1Þ ¼ 0; u3ð0; x3Þ ¼ u3ð0; L1Þ ¼ 0; φð0; x3Þ ¼ φð0; L1Þ ¼ 0 (7.145) For each layer, there are six unknowns and six continuity conditions due to u1 ¼ 0. There are also total six boundary conditions on the top and bottom surfaces. In order to satisfy Eq. (7.145) automatically, Heyliger and Brooks (1995) took the solution in the following form: ðu2; u3; φÞ ¼ u20 cos px2; u30 sin px2; φ0 sin px2ð Þesx3 eiωt ; p ¼ nπ L2= (7.146) Substituting Eq. (7.146) into (7.142) yields ÀC22p2 þ C44s2 þ ρω2 ðC23 þ C44Þps ðe24 þ e32Þps ÀðC23 þ C44Þps ÀC44p2 þ C33s2 þ ρω2 Àe24p2 þ e33s2 Àðe32 þ e24Þps Àe24p2 þ e33s2 E22p2 À E33s2 2 4 3 5 u20 u30 φ0 8 : 9 = ; ¼ 0 0 0 8 : 9 = ; (7.147) 370 7 Three-Dimensional and Applied Electroelastic Problems
33. 33. Setting the determinant of above matrix to zero for a nontrivial solution yields an eigen-equation. From the eigen-equation, we get six eigenvalues si; i ¼ 1 À 6 for s. Corresponding each si , an eigenvector U0j (u10i; u20i; u30i; φ0i ) with one unknown u10j can be obtained. As shown in Sect. 7.5.1, the problem can be solved uniquely. 7.5.4 A Mindlin-Type Plate Bending Theory Consider an orthotropic piezoelectric plate of moderate thickness. Let ðx1; x2Þ be located on the middle surface. The basic assumptions of the Mindlin bending theory are: 1. Straight lines normal to the x1 À x2 plane before deformation remain straight with unchanged length after deformation, but not compulsory normal to the mid- surface, i.e., ε11 ¼ u0 1;1 þ x3ψ1;1; ε22 ¼ u0 2;2 þ x3ψ2;2; γ23 ¼ u0 3;2 þ ψ2 γ13 ¼ u0 3;1 þ ψ1; γ12 ¼ u0 1;2 þ u0 2;1 þ x3ðψ1;2 þ ψ2;1Þ (7.148) whereu0 is the displacement in the mid-surface andψ1 andψ2 are the absolute cross- sectional rotations. 2. Stress σ33 can be neglected. So the constitutive equation can be written as σ1 ¼ σ11 ¼ C11u1;1 þ C12u2;2 þ e31φ;3; σ2 ¼ σ22 ¼ C12u1;1 þ C22u2;2 þ e32φ;3 σ4 ¼ σ23 ¼ C44ðu2;3 þ u3;2Þ þ e24φ;2; σ5 ¼ σ31 ¼ C55ðu1;3 þ u3;1Þ þ e15φ;1 σ6 ¼ σ12 ¼ C66ðu2;1 þ u1;2Þ; D1 ¼ e15ðu1;3 þ u3;1Þ À E11φ;1 D2 ¼ e24ðu2;3 þ u3;2Þ À E22φ;1; D3 ¼ e31u1;1 þ e32u2;2 À E33φ;3 (7.149) where u3;3 has been eliminated by using σ3 ¼ 0, and Cij ¼ Cij À Ci3Cj3 C33= ; eij ¼ eij À e33Cji C33= ; Eij ¼ Eij þ e2 33δi3δj3 C33= (7.150) are the reduced material coefﬁcients. Wang and Yang (2000) reviewed the higher-order theories of the piezoelectric plates. The equivalent single-layer models for the multiply layer plate (Krommer and Irschik 2000) are adopted here. Substituting Eq. (7.148) into (7.149) and 7.5 Laminated Piezoelectric Plates 371
34. 34. integrating through the thickness yield the constitutive equation in the stress resultants and moments: N1 N2 N12 M1 M2 M12 8 : 9 = ; ¼ A11 A12 0 B11 B12 0 A12 A22 0 B12 B22 0 0 0 A66 0 0 B66 B11 B12 0 D11 D12 0 B12 B22 0 D12 D22 0 0 0 B66 0 0 D 2 6 6 6 6 6 6 6 6 4 3 7 7 7 7 7 7 7 7 5 u0 1;1 u0 2;2 u0 1;2 þ u0 2;1 ψ1;1 ψ2;2 ψ1;2 þ ψ2;1 8 : 9 = ; À N1e N2e N12e M1e M2e M12e 8 : 9 = ; q2 q1 ( ) ¼ S44 0 0 S55 ! γ23 γ13 ( ) À q2e q1e ( ) (7.151) where N1; N2; N12 ¼ N6 are the membrane forces, M1; M2; M12 ¼ M6 are the bending moments, and q1; q2 are the shear forces per unit length. The generalized stiffness in Eq. (7.151) are ðNi; MiÞ ¼ XN k¼1 Z hk σ ðkÞ i 1; x3;ð Þdx3; ði ¼ 1; 2; 6Þ; ðq2; q1Þ ¼ XN k¼1 Z hk ðσ ðkÞ 4 ; σ ðkÞ 5 Þdx3 ðAij; Bij; DijÞ ¼ XN k¼1 Z hk C ðkÞ ij 1; x3; x2 3 À Á dx3; Sij ¼ XN k¼1 Z hk ΦiΦj C ðkÞ ij dx3 N1e M1e N2e M2e N12e M12e 8 : 9 = ; ¼ XN k¼1 Z hk e ðkÞ 31 e ðkÞ 32 0 8 : 9 = ; E ðkÞ 3 ð1; x3Þdx3; q1e q2e # ¼ XN k¼1 Z hk Φ2 5e ðkÞ 24 E ðkÞ 1 Φ2 4e ðkÞ 15 E ðkÞ 2 8 : 9 = ; dx3 (7.152) where Φi; Φj are shear factors which are determined by the shear stress distribution on the cross section and N1e; M1e; N2e; M2e; N12e; M12e; q1e; q2e are introduced by piezoelectric effect. The electric variables will be studied layer by layer, and for each layer, there are two-type boundary conditions: 1. Electrically open Given the electric charge density σðiÞ on the upper and lower surfaces of the layer. Usually D ðiÞ 1 and D ðiÞ 2 are neglected and D ðiÞ 3 is reserved. So D ðiÞ 3 is constant along the thickness direction due to Gauss equation D ðiÞ 3;3 ¼ 0: D ðiÞ j nj ¼ D ðiÞ 3 ¼ ÀσðiÞ ; E ðiÞ 3 ¼ ÀσðiÞ E ðiÞ 33 . (7.153) 2. Electrically shorted Given the potential VðiÞ on the upper and lower surfaces of the layer. For convenience, assume the variation of the potential is linear along the thickness direction, so E ðiÞ 3 ¼ VðiÞ hi= ; D ðiÞ 3 ¼ E ðiÞ 33VðiÞ hi= ; E ðiÞ 1 ¼ E ðiÞ 2 ¼ 0 (7.154) 372 7 Three-Dimensional and Applied Electroelastic Problems
35. 35. In Mindlin theory, the motion equations are ρ0 €u0 1 þ ρ1 €ψ1 ¼ N1;1 þ N12;2; ρ0 €u0 2 þ ρ1 €ψ2 ¼ N2;2 þ N12;1; ρ0 €u0 3 ¼ q1;1 þ q2;2 þ p ρ1 €u0 1 þ ρ2 €ψ1 ¼ M1;1 þ M12;2 À q1; ρ1 €u0 2 þ ρ2 €ψ2 ¼ M2;2 þ M12;1 À q2 (7.155) where p is the transverse loading and ðρ0; ρ1; ρ2Þ ¼ XN k¼1 Z hk ρ ðkÞ 0 1; x3; x2 3 À Á dx3 (7.156) Equations (7.148), (7.149), (7.150), (7.151), (7.152), (7.153), (7.154), (7.155), and (7.156) are the complete governing equations. For a symmetrically laminated, transversely isotropic and simply supported plate, bending and extension are decouple, and the following relations are held: C11 ¼ C22; C44 ¼ C55; C66 ¼ 1 2 C11 À C12ð Þ; e31 ¼ e32; e15 ¼ e24; E11 ¼ E22 D11 ¼ D22; D66 ¼ ðD11 À D12Þ=2; S44 ¼ S55; M1e ¼ M2e (7.157) Eliminating the cross-sectional rotations ψ from Eqs. (7.151) and (7.155) for the bending vibration, a fourth-order partial differential equation for u0 3 is obtained (Krommer and Irschik, 2000): D11r2 r2 u0 3 À D11 S44=ð Þρ0 þ ρ2½ r2 €u0 3 þ ρ0 €u0 3 þ ρ0ρ2 S44=ð Þ€u€3 0 ¼ p À ðD11 S44= Þr2 p þ ρ2 S44=ð Þ€p À r2 M1e (7.158) where r2 u0 3 ¼ u0 3;11 þ u0 3;22 and €u€3 0 ¼ @4 u0 3 @t4 . When the external loadings are p ¼ p0eiωt and M1e ¼ M10eeiωt , the frequency equation of the bending vibration is D11r2 r2 U0 3 þ ðD11 S44= Þρ0 þ ρ2½ ω2 r2 U0 3 À ρ0ω2 1 À ðρ2 S44= Þω2 Â Ã U0 3 ¼ p0 1 À ðρ2 S44= Þω2 Â Ã À r2 ðD11 S44= Þp0 þ M10e½  (7.159) where the common factor eiωt is omitted and u0 3 ¼ U0 3eiωt . 7.5.5 Third-Order Shear Deformation Theory of Laminate Plate Consider the linear piezoelectric material, so the Maxwell stress and the environment need not be considered. The variational principle δΠ ¼ 0 in Eq. (2.7) is becomes 7.5 Laminated Piezoelectric Plates 373
36. 36. δΠ ¼ Z V σikδui;kdV þ Z V Dkδφ;kdV þ Z V ρ€ukδukdV À Z aσ TÃ k δukda þ Z aρ σÃ δφda ¼ 0 (7.160) where the body force and body electric charge are neglected. For the orthotropic material of moderate thickness, Mitchell and Reddy (1995) adopted the displace- ments of the equivalent single-layer plate as u1 ¼ u0 1ðx1; x2; tÞ þ η1ðx3Þψ1ðx1; x2; tÞ À η2ðx3Þu0 3;1ðx1; x2; tÞ u2 ¼ u0 2ðx1; x2; tÞ þ η1ðx3Þψ2ðx1; x2; tÞ À η2ðx3Þu0 3;2 u3 ¼ u0 3ðx1; x2; tÞ η1ðx3Þ ¼ x3 À cx3 3; η2ðx3Þ ¼ cx3 3; c ¼ 4 3h2 (7.161) where u0 1; u0 2; u0 3 À Á are the displacements of a point on the midplane and ðψ1; ψ2Þ are the rotations of a transverse normal at x3 ¼ 0 on the midplane about the x2 and À x1 axes, respectively. h is the total thickness of the plate. The strains corresponding to Eq. (7.161) are ε11 ¼ u0 1;1 þ η1ψ1;1 À η2u0 3;11; ε22 ¼ u0 2;2 þ η1ψ2;2 À η2u0 3;22; ε33 ¼ 0 γ23 ¼ u2;3 þ u3;2 ¼ η1;3ψ2 À η2;3u0 3;2 þ u0 3;2; γ31 ¼ u1;3 þ u3;1 ¼ η1;3ψ1 À η2;3u0 3;1 þ u0 3;1 γ12 ¼ u1;2 þ u2;1 ¼ u0 1;2 þ u0 2;1 þ η1 ψ1;2 þ ψ2;1 À Á À η2 u0 3;12 þ u0 3;21 (7.162) From Eqs. (7.161) and (7.162), it is known that for η1ðx3Þ; η2ðx3Þ given in Eq. (7.161), the transverse shear strains γ13; γ23 are zeros on the upper and lower surfaces and vary quadratically through the thickness. It is also without the normal strain. The potential is modeled on a discrete layer approximation as φðx1; x2; x3; tÞ ¼ XN k¼1 Xm j¼1 fkðx3Þφðk;jÞ ðx1; x2; tÞ (7.163) where N is the layer number of the laminate plate, m is the number of interpolation points in a layer, and φðk;jÞ is the potential at jth interpolation point of kth layer. fkðx3Þ is the Lagrange interpolation function. It is noted that the potential on the upper surface of the k À 1 layer must be equal to that on the lower surface of the k layer. The middle plane is denoted by A and its boundary is L. Substituting Eqs. (7.161) and (7.163) into (7.160) and neglecting σ33 yield the following equations: 374 7 Three-Dimensional and Applied Electroelastic Problems
37. 37. The variation of the mechanical energy: Z V σikδui;kdV ¼ Z A N1δu0 1;1 þ M1δψ1;1 À P1δu0 3;11 þ N2δu0 2;2 þ M2δψ2;2 À P2δu0 3;22 n þ N6 δu0 1;2 þ δu0 2;1 þ M6 δψ1;2 þ δψ2;1 À Á À 2P6δu0 3;12 h i þ Q4 δψ2 þ δu0 3;2 þ Q5 δψ1 þ δu0 3;1 o dA ¼ À Z A N1;1δu0 1 þ M1;1δψ1 À P1;11δu0 3 À ÁÈ þ N2;2δu0 2 þ M2;2δψ2 À P2;22δu0 3 À Á þ N6;2δu0 1 þ N6;1δu0 2 þ M6;2δψ1 À þ M6;1δψ2À2P6;12δu0 3 Á þ Q4δψ2 À Q4;2δu0 3 À Á þ Q5δψ1 À Q5;1δu0 3 À ÁÉ dA þ Z L N1δu0 1 þ M1δψ1 À P1δu0 3;1 À P1;1δu0 3 h in n1 þ N2δu0 2 þ M2δψ2 À P2δu0 3;2 À P2;2δu0 3 h i n2 þ N6δu0 2 þ M6δψ2 À Á n1 þ N6δu0 1 þ M6δψ1 À Á n2 À P6δu0 3;2n1 þ P6δu0 3;1n2 À P6;1n2 þ P6;2n1 À Á δu0 3 h i þ Q4n2 þ Q5n1ð Þδu0 3 É dL (7.164) where the Voigt notation has been used and Ni ¼ Z h 2= Àh 2= σidx3; Mi ¼ Z h 2= Àh 2= σiη1dx3; Pi ¼ Z h 2= Àh 2= σiη2dx3; i ¼ 1; 2; 6 Qi ¼ Z h 2= Àh 2= σi 1 À 4ðz h= Þ2 h i dx3; i ¼ 4; 5 (7.165) The variation of the electric energy: Z V Diδφ;idV ¼ XN k¼1 Z V Xm j¼1 Dðk;jÞ α δφðk;jÞ ;α þ D k;jð Þ 3 δφ ðk;jÞ ;3 dV ( ) ¼ XN k¼1 Z A À Xm j¼1 Pðk;jÞ α;α À G ðk;jÞ 3 δφ k;jð Þ dA þ Z L Xm j¼1 Pðk;jÞ α nαδφðk;jÞ dL ( ) Pðk;jÞ α ¼ Z hj hjÀ1 Dðk;jÞ α fkðx3Þdx3; G ðk;jÞ 3 ¼ Z hj hjÀ1 D ðk;jÞ 3 fk;3ðx3Þdx3 (7.166) The variation of the kinetic energy or inertial energy: Z V ρ€uiδuidV ¼ Z A I1 €u0 1 þ I2 €ψ1 À I3 €u0 3;1 δu0 1 n þ I2 €u0 1 þ I4 €ψ1 À I5 €u0 3;1 δψ1 þ I3 €u0 1 þ I5 €ψ1 À I6 €u0 3;1 ;1 þ I3 €u0 2 þ I5 €ψ2 À I6 €u0 3;2 ;2 þ I1 €u0 3 ! δu0 3 þ I1 €u0 2 þ I2 €ψ2 À I3 €u0 3;2 δu0 2 þ I2 €u0 2 þ I4 €ψ2 À I5 €u0 3;2 δψ2 h io dA (7.167) 7.5 Laminated Piezoelectric Plates 375
38. 38. where I1 ¼ Z h 2= Àh 2= ρdx3; I3 ¼ Z h 2= Àh 2= ρη2ðx3Þdx3; I5 ¼ Z h 2= Àh 2= ρη1ðx3Þη2ðx3Þdx3 I2 ¼ Z h 2= Àh 2= ρη1ðx3Þdx3; I4 ¼ Z h 2= Àh 2= ρη2 1ðx3Þdx3; I6 ¼ Z h 2= Àh 2= ρη2 2ðx3Þdx3 (7.168) In Eq. (7.167) term À R L I3 €u0 1 þ I5 €ψ1 À I6 €u0 3;1 n1 þ I3 €u0 2 þ I5 €ψ2 À I6 €u0 3;2 n2 h i δu0 3 has been neglected. This term is difﬁcult to explanation. The variation of the work of the generalized external force is as follows: The mechanical force acted on the equivalent single-layer plate should be distinguished two parts—TÃ i is the equivalent traction on the midplane A, and tÃ i is the equivalent resultant force on the lateral surface a. The electric charge acted on the kth layer should also be distinguished two parts: σðkÞÃ is the surface electric charge density of the kth layer, and qðkÞÃ is the surface electric charge on the lateral surface. Neglecting some secondary terms we can get À Z aσ TÃ k δukda þ Z aρ σÃ δφda ¼ À Z A TÃ 1δu0 1þ È TÃ 2δu0 2 þ TÃ 3δu0 3 É dA À Z L tÃ 1δu0 1þ È tÃ 2δu0 2 þ tÃ 3δu0 3 É dL þ XN k¼1 Z A σðkÞÃ fkδφjdA þ Z L qðkÞÃ fjδφjdL ! (7.169) Substitution of Eqs. (7.163), (7.164), (7.165), (7.166), (7.167), (7.168), and (7.169) into Eq. (7.160) yields δu10 : N1;1 þ N6;2 þ TÃ 1 ¼ I1 €u0 1 þ I2 €ψ1 À I3 €u0 3;1 δu20 : N2;2 þ N6;1 þ TÃ 2 ¼ I1 €u0 2 þ I2 €ψ2 À I3 €u0 3;20 δu30 : P1;11 þ P2;22 þ 2P6;12 þ Q4;2 þ Q5;1 À TÃ 3 ¼ I3 €u0 1 þ I5 €ψ1 À I6 €u0 3;1 ;1 þ I3 €u0 2 þ I5 €ψ2 À I6 €u0 3;2 ;2 þ I1 €u0 3 δψ1 : M1;1 þ M6;2 À Q5 ¼ I2 €u0 1 þ I4 €ψ1 À I5 €u0 3;1 δψ2 : M2;2 þ M6;1 À Q4 ¼ I2 €u0 2 þ I4 €ψ2 À I5 €u0 3;2 δφðk;jÞ : Xm j¼1 Pðk;jÞ α;α À G ðk;jÞ 3 ¼ Xm j¼1 σðjÞÃ fj (7.170) 376 7 Three-Dimensional and Applied Electroelastic Problems
39. 39. and the natural boundary conditions are δu0 1 : N1n1 þ N6n2 þ tÃ 1 ¼ 0; δu0 2 : N2n2 þ N6n1 þ tÃ 2 ¼ 0 δu0 3 : P1;1n1 þ P2;2n2 þ P6;1n2 þ P6;2n þ Q4n2 þ Q5n1 þ tÃ 3 ¼ 0 δψ1 : M1n1 þ M6n2 ¼ 0; δψ2 : M2n2 þ M6n1 ¼ 0 δu0 3;1 : P1n1 þ P6n2 ¼ 0; δu0 3;2 : P2n2 þ P6n1 ¼ 0 δφk j : Xm j¼1 Pðj;kÞ α nα À qðkÞÃ fjðx3Þ ¼ 0 (7.171) It is also noted that on the boundaries given generalized displacements, we have δu0 1 ¼ δu0 2 ¼ δu0 3 ¼ δu0 3;1 ¼ δu0 3;2 ¼ δψ1 ¼ δψ2 ¼ 0 (7.172) Mitchell and Reddy (1995) adopted Hamilton principle,δΠH ¼ δΠH1 in Eq. (2.32); their results are slightly different. It can be seen that this complex approximate theory is difﬁcult to exactly discuss and give some new simpliﬁed postulations are needed. The generalized forces can be obtained from Eqs. (7.165) and (7.149). Let Ni ¼ Ni þ Np i ; Mi ¼ Mi þ Mp i ; Pi ¼ Pi þ Pp i ; Qi ¼ Qi þ Qp i (7.173a) where the elastic variables are denoted by an over-bar and variables related to piezoelectric effect are denoted by a superscript “p,” and N1 N2 N3 M1 M2 M3 P1 P2 P3 8 : 9 = ; ¼ A11 A12 0 AÃ 11 AÃ 12 0 AÃÃ 11 AÃÃ 12 0 A12 A22 0 AÃ 12 AÃ 22 0 AÃÃ 12 AÃÃ 22 0 0 0 A66 0 0 AÃ 66 0 0 AÃÃ 6 AÃ 11 AÃ 12 0 B11 B12 0 BÃ 11 BÃ 12 0 AÃ 12 AÃ 22 0 B12 B22 0 BÃ 12 BÃ 22 0 0 0 AÃ 66 0 0 B66 0 0 BÃ 66 AÃÃ 11 AÃÃ 12 0 BÃ 11 BÃ 12 0 D11 D12 0 AÃÃ 12 AÃÃ 22 0 BÃ 12 BÃ 22 0 D12 D22 0 0 0 AÃÃ 66 0 0 BÃ 66 0 0 D66 2 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 6 4 3 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 7 5 u0 1;1 u0 2;2 u0 1;2 þ u0 2;1 ψ1;1 ψ2;2 ψ1;2 þ ψ2;1 Àu0 3;11 Àu0 3;22 À2u0 3;12 8 : 9 = ; (7.173b) Q4 Q5 ( ) ¼ F44 0 0 F55 ψ2 þ u30;2 ψ1 þ u30;1 ( ) (7.173c) 7.5 Laminated Piezoelectric Plates 377
40. 40. Np 1 ¼ XN k¼1 e ðkÞ 31 Xm j¼1 β ðk;jÞ 1 φðk;jÞ ; Np 2 ¼ XN k¼1 e ðkÞ 32 Xm j¼1 β ðk;jÞ 1 φðk;jÞ ; Np 6 ¼ 0 Mp 1 ¼ XN k¼1 e ðkÞ 31 Xm j¼1 β ðk;jÞ 2 φðk;jÞ ; Mp 2 ¼ XN k¼1 e ðkÞ 32 Xm j¼1 β ðk;jÞ 2 φðk;jÞ ; Mp 6 ¼ 0 Pp 1 ¼ XN k¼1 e ðkÞ 31 Xm j¼1 β ðk;jÞ 3 φðk;jÞ ; Pp 2 ¼ XN k¼1 e ðkÞ 32 Xm j¼1 β ðk;jÞ 3 φðk;jÞ ; Pp 6 ¼ 0 Qp 4 ¼ XN k¼1 e ðkÞ 24 Xm j¼1 β ðk;jÞ 4 @φðk;jÞ @x2= ; Qp 5 ¼ XN k¼1 e ðkÞ 15 Xm j¼1 β ðk;jÞ 4 @φðk;jÞ @x1= (7.173d) where AðkÞ ¼ Z hk 2= Àhk 2= Cdx3; AðkÞÃ ¼ Z hk 2= Àhk 2= Cg1dx3; AðkÞÃÃ ¼ Z hk 2= Àhk 2= Cg2dx3; BðkÞ ¼ Z hk 2= Àhk 2= Cg2 1dx3 BðkÞÃ ¼ Z hk 2= Àhk 2= Cg1g2dx3; D ¼ Z hk 2= Àhk 2= Cg2 2dx3; F44 ¼ Z hk 2= Àhk 2= C44g2 1;3dx3 F55 ¼ Z hk 2= Àhk 2= C55g2 1;3dx3β ðk;jÞ 1 ¼ Z hk 2= Àhk 2= fj;3dx3; β ðk;jÞ 2 ¼ Z hk 2= Àhk 2= g1fj;3dx3; β ðk;jÞ 3 ¼ Z hk 2= Àhk 2= g2fj;3dx3; β ðk;jÞ 4 ¼ Z hk 2= Àhk 2= g1;3fjdx3; C ¼ C11 C12 0 C21 C22 0 0 0 C66 0 B @ 1 C A A; AÃ ; AÃÃ ; B; BÃ ð Þ ¼ XN k¼1 AðkÞ ; AðkÞÃ ; AðkÞÃÃ ; BðkÞ ; BðkÞÃ (7.174) Equations (7.170), (7.171), (7.172), (7.173a), (7.173b), (7.173c), (7.173d), and (7.174) are the complete governing equations. 7.5.6 Bending Theory of Timoshenko Beam A narrow plate can be considered as a beam. The Timoshenko theory (Timoshenko and Woinowsky-Krieger 1959) considering the shear deformation of a beam of a moderate thickness can be obtained from the Mindlin theory. Let all variables be independent to x2 in Mindlin theory, Eq. (7.149) is reduced to σ1 ¼ σ11 ¼ Yu1;1 þ e31φ;3; σ5 ¼ σ13 ¼ Gðu1;3 þ u3;1Þ þ e15φ;2 D1 ¼ e15ðu1;3 þ u3;1Þ À E11φ;1; D3 ¼ e31u1;1 À E33φ;3 (7.175) 378 7 Three-Dimensional and Applied Electroelastic Problems
41. 41. where Y; G are elastic coefﬁcients. Corresponding to Eq. (7.148), the deformation in Timoshenko beam is assumed as ε11 ¼ u0 1;1 þ x3ψ;1; γ13 ¼ u0 3;1 þ ψ (7.176) If ψ ¼ Àu0 3;1 , then γ13 ¼ 0,Timoshenko beam is reduced to Bernoulli-Euler beam. Corresponding to Eqs. (7.173) and (7.174), we have N M ( ) ¼ A B B D u0 1;1 ψ;1 ( ) À Ne Me ( ) ; q ¼ Gγ13 À qe A; B; Dð Þ ¼ XN k¼1 Z hk YðkÞ 1; x3:x2 3 À Á dx3; G ¼ XN k¼1 Z hk Φ2 GðkÞ dx3 Ne; Með Þ ¼ XN k¼1 Z hk e ðkÞ 31 E ðkÞ 3 1; x3:ð Þdx3; qe ¼ XN k¼1 Z hk Φ2 e ðkÞ 15 E ðkÞ 1 dx3 (7.177) Corresponding to Eq. (7.155), we have ρ0 €u0 1 þ ρ1 €ψ1 ¼ N;1; ρ0 €u0 3 ¼ q;1 þ p; ρ1 €u0 1 þ ρ2 €ψ1 ¼ M;1 À q (7.178) where ρ0; ρ1; ρ2 are shown in Eq. (7.156) and electric displacements and electric ﬁelds are shown in Eq. (7.153) or (7.154). 7.5.7 Bending Model of Beams of Crawley Crawley and De Luis (1987) proposed an extension-bending model to study the simple intelligent beam structure as shown in Fig. 7.8. They assumed that the strain is uniform through the actuator thickness, the beam obeys Bernoulli-Euler rule, and the adhesive layer transfers loads only through shear. The formulas obtained by this model are well for extension, but not bending, especially for a thin plate (Crawley and Aanderson 1989). 7.6 The First-Order Approximate Theory of an Electro-magneto-elastic Thin Plate 7.6.1 Basic Postulations The nonlinear theory of an electroelastic thin plate is not well established, and different authors proposed different theories. In this section, a ﬁrst-order approxi- mate theory of the quasi-static electro-magneto-elastic thin plate is recommended 7.6 The First-Order Approximate Theory of an Electro-magneto-elastic Thin Plate 379
42. 42. for small deformation, when the electromagnetic induction effect can be neglected. Let the origin of the coordinate system axes x1; x2 be located on the midplane and x3 be upward normal to the midplane. The plate is bending upward. The role of x3 is not the same as that of ðx1; x2Þ, so it will be discussed alone. For the present plate theory, three following basic postulations are assumed (Kuang 2011): (1) σ33 ( σα3 ( σαβ; ðα ¼ 1; 2Þ, so σ33 is fully neglected and the effect of σα3 is considered partly. (2) The Kirchhoff assumption is adopted, i.e., uk ¼ u0 k À x3u0 3;k; u0 k ¼ u0 kðx1; x2; tÞ; u0 k;3 ¼ 0; ðk ¼ 1; 2; 3Þ (7.179) where u0 is the displacement on the middle surface and u is the displacement at a certain point in the plate. According to Eq. (7.179), we have u3;α þ uα;3 ¼ 0, but it is not appropriate for the free boundary and should be modiﬁed approximately as shown later. (3) The electromagnetic ﬁeld obeys the 3D theory, but in order to consistent with the classical plate theory, the resultant electromagnetic force is reduced to the middle plane S (dS ¼ dx1dx2 ) or to the contour L of the middle plane. Usually when we solve the electromagnetic ﬁeld, the electric ﬁeld due to the direct piezo- electric effect can be approximately neglected compared to the lager applied electric ﬁeld. 7.6.2 Governing Equations Derived from the First Method In engineering the piezoelectric plate is surrounded by air, so the plate has only the interface with the air and does not have its own independent boundary. In air the mechanical stresses can be neglected, so only the electromagnetic ﬁeld should be considered. It is assumed that there is no body force and body electric charge. According to Eqs. (2.19) and (2.21), there are two methods to establish the thin plate theory. Similar to Eq. (2.36), the ﬁrst alternative form of the PVP, Eq. (2.19), for the static electromagnetic problem is modiﬁed as δ^Π ¼ δ^Π1 þ δ^Π2 À δWint ¼ Z V Sklδuk;ldV þ Z V ρ€ukδukdV À Z aint σ TÃ int k δukda þ Z V Dkδφ;kdV þ Z V Bkδψ;kdV þ Z Vair Dair k δφair ;k dV þ Z Vair σM air kl δuair k;ldV þ Z Vair Bair k δψair ;k dV À Z aair μ BÃair i nair i δψair da Skl ¼ σkl þ σM kl ; σM ik ¼ DiEk þ BiHk À 1 2=ð Þ DnEn þ BnHnð Þδik (7.180) Sair kl has the similar expression. The mechanical part related to the plate of the PVP is 380 7 Three-Dimensional and Applied Electroelastic Problems
43. 43. Z aint σ Skl À σM air kl À Á nl À TÃ int k Â Ã δukda À Z V Skl;l À ρ€uk À Á δukdV ¼ 0 (7.181) Therefore, the thin plate theory can apply the usual elastic plate theory, but σ is replaced bySand on the interfaceTÃ int is replaced byTÃ int þ σM air Á n. According to the textbook of elastic plate theory, the bending theory of elastic electromagnetic thin plate can be expressed as Field equation: M ðSÞ αβ;βα þ qÃ ¼ 0; in S (7.182) Boundary conditions: Clamped side u0 3 ¼ u0Ã 3 ; u0 3;n ¼ u0Ã 3;n (7.183a) Hinged side u0 3 ¼ u0Ã 3 ; MðSÞ n ¼ MÃ n þ MM air n ; (7.183b) Free side M ðSÞ nt;t þ QðSÞ n ¼ QÃ n þ QM air n ; MðSÞ n ¼ MÃ n þ MM air n (7.183c) The notations in Eqs. (7.182) and (7.183) are M ðSÞ αβ ¼ Z h Àh Sαβx3dx3; MM air n ¼ MM air α nα; MM air α ¼ Z h Àh σM air αβ x3dx3 QðSÞ α ¼ Z h Àh Sα3dx3; QðSÞ n ¼ QðSÞ α nα; QM air α ¼ Z h Àh σM air α3 dx3 (7.184) where 2h is the thickness of the plate, qÃ is the distributed loading on the plate surface, and QÃ n is the distributed loading on the lateral boundary of the midplane. At ﬁrst the electromagnetic ﬁelds in plate and air are solved under the assumption that the elastic effect can be neglected. After solving the electromagnetic ﬁelds, the entire problem is reduced to a linear problem. 7.6.3 Governing Equations Derived from the Second Method Similar to Eq. (2.36), the second alternative form of the PVP, Eq. (2.21), for the static electromagnetic problem is modiﬁed as δΠ0 ¼ δΠ0 1 þ δΠ0 2 À δW0int ¼ Z V σklδuk;ldV À Z V σM jk;j À ρ€uk δukdV À Z aint σ Tint Ã k þ σM env jk nenv j À σM jk nj δukda þ Z V Dkδφ;kdV þ Z V Bkδψ;kdV þ Z Venv Denv k δφenv ;k dV þ Z aenv D σenv Ã δφenv da þ Z Venv Benv k δψenv ;k dV À Z Venv σM env jk;j δuenv k dV þ Z aD σÃ δφda À Z aenv μ Bi Ãenv nenv i δψenv da ¼ 0 σM ik ¼ DiEk þ BiHk À 1 2=ð Þ DnEn þ BnHnð Þδik; Similar expression for σM env ik (7.185) 7.6 The First-Order Approximate Theory of an Electro-magneto-elastic Thin Plate 381
44. 44. According to postulation (3), the electromagnetic ﬁeld obeys the 3D theory, which has been discussed in Chap. 2. Here only the mechanical part related to the plate of the variational principle is discussed in detail, which is Z V σklδuk;ldV À Z V σM jk;j À ρ€uk δukdV À Z aint σ Tint Ã k þ σM env jk nenv j À σM jk nj δukda (7.186) Applying postulations (1) and (2) and noting n3 ¼ 1; nα ¼ 0 on the midplane, n3 ¼ 0 on the lateral surface, it is obtained: Z V σklδul;kdV ¼ Z L Nαβnβδu0 αdL À Z s Nαβ;βδu0 αds À Z L Mαβnβδu0 3;αdL þ Z L Mαβ;αnβδu0 3dL À Z s Mαβ;βαδu0 3ds Z V ρ€ukδukdV ¼ Z s ρ0 €u0 3 þ ρ1 €u0 α;α À ρ2u0 3;αα δu0 3ds þ Z s ρ0 €u0 α À ρ1 €u0 3;α δu0 αds À Z L ρ1 €u0 k À ρ2u0 3;k nkδu0 3dL Z aint σM ip niδupda ¼ Z L NM αpnαδu0 pdL À Z L MM αβnαδu0 3;βdL þ Z S pM i δu0 i dS Z V σM ip;iδupdV ¼ Z s NM iα;iδu0 αdS À Z L MM iα;inαδu0 3dL þ Z s MM iα;iαδu0 3dS þ Z s NM i3;iδu0 3dS Z aint σ TÃint l δulda ¼ Z S pÃint l δu0 l dS þ Z Lσ PÃint l δu0 l dL À Z Lσ MÃint l δu0 3;ldL (7.187) where 2h is the thickness of the plate. The expression of σM air ip is similar to σM ip. The notations in Eq. (7.187) are Nαβ ¼ Z h Àh σαβdx3; Mαβ ¼ Z h Àh σαβx3dx3; NM αp ¼ Z h Àh σM αpdx3; MM αp ¼ Z h Àh σM αpx3dx3 pM i ¼ NM 3i;3 ¼ Z h Àh σM 3i;3dx3 ¼ σM 3i ðhÞ À σM 3i ðÀhÞ; MM 3i;3 ¼ Z h Àh σM 3i;3x3dx3 ρ0 ¼ Z h Àh ρdx3; ρ1 ¼ Z h Àh ρx3dx3; ρ2 ¼ Z h Àh ρx2 3dx3; pÃint l ¼ TÃint l h Àh ; on S; PÃint l ¼ Z h Àh TÃint l dx3; MÃint l ¼ Z h Àh TÃint l x3dx3; on L (7.188) It is noted that when the Maxwell stresses on the upper and lower surfaces are reduced to the midplane, a distributed couple R S mM 3α À mM env 3α À Á δu0 3;αdS; mM 3α ¼ σM 3αðhÞ þ σM 3α Àhð Þ Â Ã h 2=ð Þ may be produced, but this effect is neglected in 382 7 Three-Dimensional and Applied Electroelastic Problems
45. 45. Eq. (7.187) due to smallh. It is also noted that Eq. (7.179) is not fully appropriate for the free lateral boundary. In fact from the variational formula, σα3 on the middle plane is approximately considered by Pint Ã 3 , but σα3 on the free boundary should not be considered. So on the boundaryL, a termN3β ¼ Rh Àh σβ3dx3 should be added to the variational formula. Substituting Eqs. (7.187) into Eq. (7.186), adding a term R L N3βnβδu0 3dL, and ﬁnishing the variational calculation, we ﬁnally get: The mechanical governing equations of the plane problem are Nαβ;β þ NM αβ;β þ pM env α À pM α þ pÃint α ¼ ρ0 €u0 α Àρ1 €u0 3;α ; in S Nαβ þ NM αβ À NM env αβ nβ ¼ PÃint α ; on Lσ (7.189) The mechanical governing ﬁeld equation for the bending problem is Mαβ;βα þ MM αi;αi þ NM α3;α þ pM env 3 À pM 3 þ pÃint 3 ¼ ρ0 €u0 3 þ ρ1 €u0 α;α À ρ2u0 3;αα ; in S Z L Mαβ;α þ MM αβ;α nβ À PÃint 3 þ N3β þ NM β3 À NM env β3 nβ À ρ1 €u0 k À ρ2u0 3;k h i δu0 3dL À Z L Mαβnβ þ MM βα À MM env βα nβ À MÃint α h i δu0 3;αdL ¼ 0 (7.190) In Eq. (7.190) terms ρ1 €u0 α;α À ρ2u0 3;αα and ρ1 €u0 k À ρ2u0 3;k can be neglected. The usual three boundary conditions for the plate bending can easily be derived from Eq. (7.190). According to the assumption (3), the electromagnetic ﬁeld is reduced to Di;i ¼ ρe; Bi;i ¼ 0; in V; Dini ¼ ÀσÃ ; on aD; Bi ¼ BÃ i ; on aμ Di À Denv i À Á ni ¼ ÀσÃint ; Bi À Benv i À Á ¼ Bi Ãint ; on aint (7.191) In deriving the above equations, the constitutive equations were not used, so the governing equations can be used for all materials satisfying the basic postulations (1) to (3). 7.6.4 Some Discussions The soft electromagnetic plate under a uniform transverse magnetic ﬁeld can be bending or buckling when the magnetic ﬁeld exceeds a critical value (Moon and Pao 1968; Pao and Yeh 1973). The natural frequency of a soft electromagnetic plate 7.6 The First-Order Approximate Theory of an Electro-magneto-elastic Thin Plate 383
46. 46. can be changed under a longitudinal magnetic ﬁeld (Zhou and Miya 1998). Zhou and Zheng (1997) pointed out that there was not a uniﬁed theory to discuss the above two problems, and they proposed a variational method attempting to uniﬁed deal with these problems. The key problem is to get the electromagnetic force acting on the plate. Though for the electromagnetically static problem and the problem without magnetic ﬁeld the theory discussed above is appropriate, but for a MQS system (@D @t= ¼ 0; @B @t= 6¼ 0), such as vibration problem in a magnetic ﬁeld, it should be modiﬁed, the motional electric force should be considered. As an example, the transverse vibration of an elastic electroconductive plate is subjected to the external uniform magnetic ﬁeld H0 ¼ H01i1 þ H02i2 parallel to the ðx1; x2Þ plane only. The induced motional electric ﬁeld e; b; j in the plate due to the plate motion is (Librescu et al. 2004; Belubekyan et al. 2007) e ¼ Àv Â B0; v ¼ v i3; b ¼ — Â ðu Â B0Þ; j ¼ — Â h (7.192) The corresponding Maxwell stress is σM ij ¼ σM0 ij þ σM1 ij σM0 ij ¼ B0iH0j À ð1 2= ÞB0mH0mδij; σM1 ij ¼ biH0j þ B0ihj À B0mhmδij (7.193) Belubekyan et al. (2007) adopted the electromagnetic body force f ¼ — Á σM , but Librescu et al. (2004) adopted the Lorentz formula f ¼ j Â B0 . The MQS problems should be further studied. 7.7 Piezoelectric Composite Shells 7.7.1 First-Order Shear Deformation Theory Consider a ﬁnite, simply supported, N-layered laminated circular cylindrical shell of mean radius R, length L, and thickness H. The shell is constituted of elastic orthotropic or radially polarized piezoelectric materials. The cylindrical coordi- nates ðx; θ; zÞ are adopted with ðx; θÞ spanning the mid-surface and z along the normal (radial) direction. Analogous to the Mindlin plate theory, Kapuria et al. (1998) assumed that the displacements can be approximated as u ¼ u0 ðx; θÞ þ zψ1ðx; θÞ; v ¼ v0 ðx; θÞ þ zψ2ðx; θÞ; w ¼ w0 ðx; θÞ (7.194) where u0 ; v0 ; w0 are the displacement components on the mid-surface and ψ1; ψ2 are the rotations of its normal. The corresponding strains are εx ¼ u0 ;x þ zψ1;x; εθ ¼ v0 ;θ þ þzψ2;θ þ w0 . ðR þ zÞ; εz ¼ 0; γzx ¼ ψ1 þ w0 ;x γθz ¼ ψ2 þ w0 ;θ À v0 À zψ2 . ðR þ zÞ; γθx ¼ v0 ;x þ u0 θ þ zψ1;θ À Á ðR þ zÞ= þ zψ2;x (7.195) 384 7 Three-Dimensional and Applied Electroelastic Problems
47. 47. On the mid-surface, the resultant membrane forces Nx; Nθ; Nxθ; Nθx, transverse forces Qx; Qθ, and resultant moments Mx; Mθ; Mxθ; Mθx are Nx; Nθ; Nxθ; Nθx Mx; Mθ; Mxθ; Mθx # ¼ Z H 2= ÀH 2= 1 z # σx 1 þ z R ; σθ; σxθ 1 þ z R ; σθx h i dz Qx; Qθ½  ¼ Z H 2= ÀH 2= σxz 1 þ z R=ð Þ; σθz½ dz (7.196) The constitutive equation is shown in Eq. (7.149). The equilibrium equations are Nx;x þ Nθx;θ R= þ px ¼ 0; ðQθ þ Nθ;θÞ R= þ Nxθ;x þ pθ ¼ 0; Qx;x þ ðQθ;θ À NθÞ R= þ pz ¼ 0 Mx;x þ Mθx;θ R= À Qx þ mx ¼ 0; Mθ;θ R= þ Mxθ;x À Qθ þ mθ ¼ 0 px; pθ; pzð Þ ¼ ð1 þ z=RÞðσzx; σzθ; σzÞ½  H 2= ÀH 2= ; ðmx; mθÞ ¼ ð1 þ z=RÞzðσzx; σzθÞ½  H 2= ÀH 2= (7.197) where px; pθ; pz; mxmθ are the external forces and moments, respectively. The boundary conditions are deﬁned: Nx or u0 ; Nxθ or v0 ; Qx or w0 ; Mx or ψ1; Mxθ or ψ2; at x ¼ 0 or L Nθx or u0 ; Nθ or v0 ; Qθ or w0 ; Mθx or ψ1; Mθ or ψ2; at θ ¼ 0 or θ0 (7.198) where θ0 is the span of the cylindrical panel. Usually σz can be neglected. Using Eqs. (7.149) and (7.150), the equilibrium equations in terms of displacements can be obtained. Here it is omitted. The above theory is easily extended to the combined multiply layer shell. The electric potential φ is assumed to vary linearly across the actuated layer, and the electric ﬁeld is computed as Ex ¼ Àφ;x; Eθ ¼ Àφ;θ ðR þ zÞ= ; Ez ¼ Àφ;z. For the classical shell theory, the transverse shear strains γzx; γθz are neglected. Hence, u ¼ u0 À zw0 ;x; v ¼ v0 À z w0 ;θ À v0 . R; w ¼ w0 ðx; θÞ; εx ¼ u0 ;x À zw0 ;xx; εθ ¼ v0 ;θ . R þ w0 À zw0 ;θθ . ðR þ zÞ; εz ¼ 0; γθx ¼ v0 ;x þ u0 θ þ zψ1;θ À Á ðR þ zÞ= þ zψ2;x; ψ1 ¼ Àw0 ;x; ψ2 ¼ v0 À w0 ;θ . R (7.199) 7.7 Piezoelectric Composite Shells 385
48. 48. The above thin shell theories yield poor predictions of the transverse stress components σxz; σθz; σz, so sometimes a post-processing technique is needed. The transverse stress can approximately be obtained from the 3D equilibrium equations (Kapuria et al. 1998): ðR þ zÞ2 σθz ¼ À Z z Àh 2= ðR þ zÞσθ;θ þ ðR þ zÞ2 σθx;x h i dz þ c1 ðR þ zÞ2 σxz ¼ À Z z Àh 2= σθx;θ þ ðR þ zÞσx;x Â Ã dz þ c2 ðR þ zÞ2 σz ¼ À Z z Àh 2= σθ À σzθ;θ À ðR þ zÞσzx;x Â Ã dz þ c3 (7.200) where ci is determined by the boundary conditions at the outer shell surface. Kapuria et al. (1998) compared the numerical results of the shell theory with that of the exact 3D theory and gave some comments. Saviz et al. (2007) proposed a layerwise model which is formulated by introducing piecewise continuous approximations through the thickness for each state variables. They showed that the results calculated by this model more consist with that from the 3D theory. 7.7.2 The Cylindrical Bending of a Laminated Inﬁnitely Long Shell The exact analytical solution of a cylindrical shell by 3D theory is difﬁcult, but for some simpler cases, it is possible. Now discuss an inﬁnitely long laminated orthotropic cylindrical shell with simple supported edges under purely cylindrical bending. The top and bottom layers are piezoelectric actuators, and the middle layer is an elastic orthotropic substrate. The cylindrical coordinates r; θ; z are used, where r; θ and z refer to the radial, circumferential, and axial directions, respectively, and ur; uθ and uz are the corresponding displacements (Fig. 7.10). Because the shell is inﬁnitely long, variables can be considered as the functions of ðr; θÞ only. The equilibrium, geometric, and constitutive equations are, respectively, σr;r þ σrθ;θ r= þ ðσr À σθÞ r= ¼ 0; σrθ;r þ σθ;θ r= þ 2σrθ r= ¼ 0 Dr þ rDr;r þ Dθ;θ ¼ 0 (7.201) εr ¼ ur;r; εθ ¼ ðuθ;θ þ urÞ=r; γrθ ¼ ður;θ À uθÞ r= þ uθ;r Er ¼ Àφ;r; Eθ ¼ Àφ;θ r= (7.202) σr ¼ C11εr þ C12εθ À e33Er; σθ ¼ C12εr þ C22εθ À e31Er σrθ ¼ C66γrθ À e15Eθ; Dr ¼ e33εr þ e31εθ þ Er Er; Dθ ¼ e15γrθ þ EθEθ (7.203) 386 7 Three-Dimensional and Applied Electroelastic Problems
49. 49. where Cij is the reduced material coefﬁcients. The boundary conditions are 1. Simply supported ur ¼ σθ ¼ σθz ¼ 0; φ ¼ 0; when θ ¼ 0; θ0 2. On the interfaces ur; uθ; σr; σrθ continuous and φ ¼ 0 (7.204) 3. Upper surface of the outer actuator σr ¼ q0 sin pθ; σrθ ¼ 0; φ ¼ V sin pθ 4. Lower surface of the inner actuator σr ¼ σrθ ¼ 0; Dr ¼ 0 where p ¼ mπ θ0= ,m is an integer, and V and q0 are given values. In order to satisfy the boundary conditions ur ¼ σθ ¼ φ ¼ 0 on the edges, Chen et al. (1996) adopted the following generalized displacements for actuators: ur ¼ u0 r ðrÞ sin pθ; uθ ¼ u0 θðrÞ cos pθ; φ ¼ φ0 ðrÞ sin pθ (7.205) Substitution of Eq. (7.205) into Eq. (7.201) for actuators yields C11 u00 r0 þ u0 r0 r À C22 þ p2 C66 À Á ur0 r2 À p C66 þ C12ð Þ u0 θ0 r þ p C22 þ C66ð Þ uθ0 r2 À e31 φ0 0 r ¼ 0 p C12 þ C66ð Þ u0 r0 r þ p C22 þ C66ð Þ ur0 r2 þ C66 u00 θ0 þ u0 θ0 r À p2 C22 þ C66 À Á uθ0 r2 þ pe31 φ0 0 r ¼ 0 e31 u0 r0 r À pe31 u0 θ0 r À Er φ00 0 þ φ0 0 r þ p2 Eθ φ0 r2 ¼ 0 (7.206) where f0 ¼ f;r; f00 ¼ f;rr for any f. Let ur0ðrÞ ¼ Arrs ; uθ0ðrÞ ¼ Aθrs ; φ0ðrÞ ¼ Aφrs (7.207) Substitution of Eq. (7.207) into Eq. (7.206) for actuators yields the homogeneous equation of Ar; Aθ; Aφ . In order to have nontrivial solutions for Ar; Aθ; Aφ , the coefﬁcient determinate of them must be zero, so the following character equation is obtained: Fig. 7.10 Cylindrical bending of an inﬁnitely long shell 7.7 Piezoelectric Composite Shells 387
50. 50. As6 þ Bs4 þ Cs2 þ D ¼ 0 A ¼ ÀC11C66 Er B ¼ C11 p2 C22 þ C66 À Á þ C66 C22 þ p2 C66 À Á À p2 C12 þ C66ð Þ2 h i Er þ p2 C11C66 Eθ þ C66 þ p2 C11 À Á e2 31 C ¼ À C22 þ p2 C66 À Á p2 C22 þ C66 À Á þ p2 C22 þ C66ð Þ2 h i Er þ p4 C12 þ C66ð Þ2 h Àp2 C11 p2 C22 þ C66 À Á À p2 C66 C22 þ p2 C66 À ÁÃ Eθ þ 2p2 C22 þ C66ð Þ Â À p2 C22 þ C66 À Á e2 31 À p2 C22 þ p2 C66 À ÁÃ e2 31 D ¼ p2 p2 C22 þ C66 À Á C22 þ p2 C66 À Á À p4 C22 þ C66ð Þ2 h i Eθ (7.208) From Eq. (7.208) s has 6 real roots sj; j ¼ 1 À 6 for piezoelectric material. For each sj, a group ðArj; Aθj; AφjÞ with one unknown is obtained, so the general solution of Eq. (7.206) for each actuator is ur0 ¼ X6 j¼1 Ajrsj ; uθ0 ¼ X6 j¼1 AjHθjrsj ; φ0 ¼ X6 j¼1 AjHφjrsj Hθj ¼ À p C12 þ C66ð Þsj þ C22 þ C66ð Þ Â Ã ÀErs2 j þ p2 Eθ À pe2 31s2 j n o. Δ Hφj ¼ À C66s2 j À p2 C22 À C66 þ p2 C12 þ C66ð Þsj þ C22 þ C66 Â Ãn o e31sj . Δ Δ ¼ C66s2 j À p2 C22 À C66 ÀErs2 j þ p2 Eθ þ pe2 31s2 j (7.209) The governing equations of the middle orthotropic composite matrix can be obtained if the electric variables in Eq. (7.206) are omitted. Let the generalized displacements in matrix be uðmÞ r ¼ arrs sin pθ; u ðmÞ θ ¼ aθrs ðrÞ cos pθ (7.210) The character equation of ar; aθ is B0 s4 þ C0 s2 þ D0 ¼ 0 B0 ¼ C11C66 C0 ¼ ÀC66ðC22 þ p2 C66Þ À C11 p2 C22 þ C66 À Á þ p2 C12 þ C66ð Þ2 D0 ¼ C22 þ p2 C66 À Á p2 C22 þ C66 À Á À p2 C12 þ C66ð Þ2 (7.211) 388 7 Three-Dimensional and Applied Electroelastic Problems
51. 51. where the superscript M of CM ij is omitted. So the solution of the substrate is ur0 ¼ X4 j¼1 ajHrjrsj ; uθ0 ¼ X4 j¼1 ajrsj Hrj ¼ p ðC12 þ C66Þsj À ðC22 þ C66Þ Â Ã C11s2 j À ðC22 þ p2 C66Þ h i. (7.212) There are 16 unknowns: 6 Aj of the outer actuator, 6 Aj of the inner actuator, and 4 aj of the middle substrate. There are also 16 boundary conditions: 4 conditions on each interface, 3 conditions on upper surface, 3 conditions on lower surface, and σθz ¼ 0 at θ ¼ 0; θ0. Therefore, the problem is solved. 7.7.3 Approximate Theory of a Functionally Graded Shallow Piezoelectric Shell Figure 7.11 shows a functionally graded shallow piezoelectric shell of thickness 2h; ðα1; α2Þ are the orthogonal curvilinear coordinates on the mid-surface; and its corresponding Lame´ parameters are H1; H2 and radii of curvatures are R1; R2. α3 is a linear coordinate and normal to the mid-surface. For a thin shell, h ( Ri; ði ¼ 1; 2Þ , Ri is approximately independent of α3 . Let ðu1; u2; u3; φÞ be the generalized displacements in the orthogonal curvilinear coordinates, then ε11 ¼ @u1 H1@α1 þ u2@H1 H1H2@α2 þ u3 R1 ; ε22 ¼ @u2 H2@α2 þ u1@H2 H1H2@α1 þ u3 R2 ε33 ¼ @u3 @α3 ; γ23 ¼ @u2 @α3 þ @u3 H2@α2 À u2 R2 ; γ13 ¼ @u1 @α3 þ @u3 H1@α1 À u1 R1 γ12 ¼ @u1 H2@α2 þ @u2 H1@α1 À u2@H2 H1H2@α1 À u1@H1 H1H2@α2 E1 ¼ À @φ H1@α1 ; E2 ¼ À @φ H2@α2 ; E3 ¼ À @φ @α3 (7.213) Fig. 7.11 Shallow piezoelectric shell 7.7 Piezoelectric Composite Shells 389
52. 52. Let CijklðzÞ; ekijðzÞ; EijðzÞ, z α3. Wu et al. (2002) assumed u1 ¼ u0 1ðα1; α2Þ þ zu1 1ðα1; α2Þ; u2 ¼ u0 2ðα1; α2Þ þ zu1 2ðα1; α2Þ u3 ¼ u0 3ðα1; α2Þ þ zu1 3ðα1; α2Þ; φ ¼ φ0 ðα1; α2Þ þ zφ1 ðα1; α2Þ þ z2 φð2Þ ðα1; α2Þ (7.214) Substitution of Eq. (7.214) into Eq. (7.213) yields the generalized strains, then substitutes the strains into the variational formula Eq. (7.160). Approximately take 1 þ z R1= % 1; 1 þ z R2= % 1. Noting dV ¼ H1H2dα1dα2dz and ﬁnishing the varia- tional calculation, the approximate equations of the thin shell can be obtained. The generalized momentum equation is δu0 1 : @ðH2N11Þ @α1 þ @ðH1N12Þ @α2 þ N12 @H1 @α2 À N22 @H2 @α1 þ N31 H1H2 R1 þ H1H2 TÃþ 1 þ TÃÀ 1 À Á ¼ H1H2 ρ0 €u0 1 þ ρ1 €u1 1 À Á δu0 2 : ðH2N12Þ;1 þ ðH1N22Þ;2 þ N12H2;1 À N11H1;2 þ N32H1H2 R2= þ H1H2 TÃþ 2 þ TÃÀ 2 À Á ¼ H1H2 ρ0 €u0 2 þ ρ1 €u1 2 À Á δu0 3 : H2N13ð Þ;1 þ ðH1N32Þ;2 À N11H1H2 R1= À N22H1H2 R2= þ H1H2 TÃþ 3 þ TÃÀ 3 À Á ¼ H1H2 ρ0 €u0 3 þ ρ1 €u1 3 À Á 3 δu1 1 : ðH2M11Þ;1 þ ðH1M12Þ;2 þ M12H1;2 À M22H2;1 þ M31H1H2 R1= À N13H1H2 þ H1H2 hTÃþ 1 À hTÃÀ 1 À Á ¼ H1H2 ρ1 €u0 1 þ ρ2 €u1 1 À Á δu1 2 : ðH2M12Þ;1 þ ðH1M22Þ;2 þ M12H2;1 À M11H1;2 þ M32H1H2 R2= À N23H1H2 þ H1H2 hTÃþ 2 À hTÃÀ 2 À Á ¼ H1H2 ρ1 €u0 2 þ ρ2 €u1 2 À Á δu1 3 : ðH2M13Þ;1 þ ðH1M23Þ;2 À M11H1H2 R1= À M22H1H2 R2= À N33H1H2 þ H1H2 hTÃþ 3 À hTÃÀ 3 À Á ¼ H1H2 ρ1 €u0 3 þ ρ2 €u1 3 À Á δφ0 : H2D0 1 À Á ;1 þ H1D0 2 À Á ;2 þ H1H2 σÃþ 1 þ σÃÀ 1 À Á ¼ 0 δφ1 : H2D1 1 À Á ;1 þ H1D1 2 À Á ;2 À H1H2D0 3 þ H1H2 hσÃþ 1 À hσÃÀ 1 À Á ¼ 0 δφð2Þ : H2D ð2Þ 1 ;1 þ H1D ð2Þ 2 ;2 À H1H2D1 3 þ H1H2 h2 σÃþ 1 À h2 σÃÀ 1 À Á ¼ 0 (7.215) The natural boundary conditions are δu0 1 : N11n1 þ N12n2 ¼ T1; δu0 2 : N12n1 þ N22n2 ¼ T2 δu0 3 : N13n1 þ N32n2 ¼ T3; δu1 1 : M11n1 þ M12n2 ¼ M1 δu1 2 : M12n1 þ M22n2 ¼ M2; δu1 3 : M13n1 þ M23n2 ¼ M3 δφ0 : D0 1n1 þ D0 2n2 ¼ Àσ0Ã ; δφ1 : D1 1n1 þ D1 2n2 ¼ Àσ1Ã δφð2Þ : D ð2Þ 1 n1 þ D ð2Þ 2 n2 ¼ Àσ2Ã (7.216) Let TÃþ i and TÃÀ i denote the traction on the upper and lower surfaces, respectively, and 390 7 Three-Dimensional and Applied Electroelastic Problems